#------------------------------------------------------------------------------
#$Date: 2016-02-13 14:50:18 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176428 $
#$URL: svn://www.crystallography.net/cod/cif/4/12/41/4124128.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4124128
loop_
_publ_author_name
'Deng, Yue'
'Eames, Christopher'
'Chotard, Jean-Noël'
'Lalère, Fabien'
'Seznec, Vincent'
'Emge, Steffen'
'Pecher, Oliver'
'Grey, Clare P.'
'Masquelier, Christian'
'Islam, M. Saiful'
_publ_section_title
;
 Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in
 Li4SiO4-Li3PO4 Solid Electrolytes.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9136
_journal_page_last               9145
_journal_paper_doi               10.1021/jacs.5b04444
_journal_volume                  137
_journal_year                    2015
_chemical_formula_sum            'Li4 O4 Si'
_chemical_formula_weight         119.85
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.0580(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            14
_cell_length_a                   11.5556(4)
_cell_length_b                   6.0986(2)
_cell_length_c                   16.7300(5)
_cell_measurement_temperature    293(2)
_cell_volume                     1164.31(7)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker D8 Venture APEXII'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0282
_diffrn_reflns_av_sigmaI/netI    0.0283
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -35
_diffrn_reflns_number            49096
_diffrn_reflns_theta_full        49.17
_diffrn_reflns_theta_max         49.17
_diffrn_reflns_theta_min         2.32
_exptl_absorpt_coefficient_mu    0.540
_exptl_crystal_density_diffrn    2.393
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             812
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.13
_refine_diff_density_max         1.198
_refine_diff_density_min         -1.189
_refine_diff_density_rms         0.136
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.901
_refine_ls_matrix_type           full
_refine_ls_number_parameters     331
_refine_ls_number_reflns         12402
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.901
_refine_ls_R_factor_all          0.0775
_refine_ls_R_factor_gt           0.0408
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1221
_refine_ls_wR_factor_ref         0.1492
_reflns_number_gt                7938
_reflns_number_total             12402
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja5b04444_si_002.cif
_cod_data_source_block           Li4SiO4
_cod_depositor_comments
'Adding full bibliography for 4124125--4124128.cif.'
_cod_original_sg_symbol_H-M      'P 21/m'
_cod_database_code               4124128
#BEGIN Tags that were not found in dictionaries:
_publcif_datablock.id            {f64d6a86-4e12-4441-aeca-efe3daffc3db}
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
#END Tags that were not found in dictionaries
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Li1 Li 0.07168(19) 0.5029(4) 0.36143(15) 0.0822(13) Uani 1 1 d .
Li2 Li 0.47613(12) 0.4947(2) 0.38281(8) 0.0111(2) Uani 1 1 d .
Li3 Li 0.72872(16) 0.7500 0.19638(11) 0.0131(3) Uani 1 2 d S
Li4 Li 0.33403(11) 0.4647(2) 0.23295(8) 0.0126(2) Uani 1 1 d .
Li5 Li 0.61647(11) 0.4973(2) 0.09223(8) 0.0114(2) Uani 1 1 d .
Li6 Li 0.72847(18) 0.2500 0.63967(12) 0.0173(4) Uani 1 2 d S
Li7 Li -0.05060(12) 0.5306(2) 0.20603(8) 0.0150(2) Uani 1 1 d .
Li8 Li 0.41018(16) 0.2500 0.51674(11) 0.0120(3) Uani 1 2 d S
Li9 Li 0.80825(12) -0.0318(2) 0.48644(8) 0.0150(2) Uani 1 1 d .
Li10 Li 0.66257(11) 0.9924(2) 0.32708(8) 0.0112(2) Uani 1 1 d .
Li11 Li 0.54666(16) 0.2500 0.22295(11) 0.0128(3) Uani 1 2 d S
Li12 Li 0.86609(19) 0.2500 0.35630(12) 0.0177(4) Uani 1 2 d S
Li13 Li 0.1437(2) 0.7500 0.23239(13) 0.0249(4) Uani 1 2 d S
Li14 Li 0.23859(12) 0.5393(2) 0.09751(8) 0.0172(3) Uani 1 1 d .
Li15 Li -0.02853(19) 0.7500 -0.07061(11) 0.0173(4) Uani 1 2 d S
Li16 Li 0.81198(12) -0.0031(2) 0.04586(8) 0.0119(2) Uani 1 1 d .
Li17 Li 0.41767(19) 0.7500 0.04749(14) 0.0225(4) Uani 1 2 d S
Li18 Li -0.0059(2) 0.2500 0.48902(15) 0.0331(6) Uani 1 2 d S
Li19 Li 1.1283(3) 0.2500 0.20945(16) 0.0406(7) Uani 1 2 d S
Si1 Si 0.38486(2) 0.2500 0.070857(14) 0.00533(4) Uani 1 2 d S
O11 O 0.52376(5) 0.2500 0.10435(4) 0.00944(10) Uani 1 2 d S
O12 O 0.34592(4) 0.47087(7) 0.01827(3) 0.00766(7) Uani 1 1 d .
O13 O 0.30522(6) 0.2500 0.14650(4) 0.00822(9) Uani 1 2 d S
Si2 Si 0.47666(2) 0.7500 0.213744(14) 0.00540(4) Uani 1 2 d S
O21 O 0.55497(6) 0.7500 0.14117(4) 0.00819(9) Uani 1 2 d S
O22 O 0.33348(5) 0.7500 0.17624(4) 0.00849(10) Uani 1 2 d S
O23 O 0.49777(4) 0.52937(7) 0.26948(3) 0.00752(7) Uani 1 1 d .
Si3 Si 0.24637(2) 0.2500 0.361532(15) 0.00585(4) Uani 1 2 d S
O31 O 0.38174(5) 0.2500 0.40108(4) 0.00835(10) Uani 1 2 d S
O32 O 0.21388(4) 0.46726(8) 0.30319(3) 0.00941(7) Uani 1 1 d .
O33 O 0.15437(6) 0.2500 0.42762(4) 0.00841(10) Uani 1 2 d S
Si4 Si 0.65890(2) 0.2500 0.493309(14) 0.00562(4) Uani 1 2 d S
O41 O 0.58026(6) 0.2500 0.56588(4) 0.00778(9) Uani 1 2 d S
O42 O 0.64167(4) 0.47293(7) 0.43938(3) 0.00790(7) Uani 1 1 d .
O43 O 0.79926(5) 0.2500 0.53783(4) 0.00935(10) Uani 1 2 d S
Si5 Si 0.79943(2) 0.2500 0.208656(14) 0.00572(4) Uani 1 2 d S
O51 O 0.71768(6) 0.2500 0.27912(4) 0.00806(9) Uani 1 2 d S
O52 O 0.78392(4) 0.47297(7) 0.15469(3) 0.00811(7) Uani 1 1 d .
O53 O 0.93847(6) 0.2500 0.25579(4) 0.00947(10) Uani 1 2 d S
Si6 Si 0.89450(2) 0.7500 0.356180(14) 0.00578(4) Uani 1 2 d S
O61 O 0.76111(5) 0.7500 0.31253(4) 0.00817(9) Uani 1 2 d S
O62 O 0.92578(4) 0.53309(8) 0.41527(3) 0.00931(7) Uani 1 1 d .
O63 O 0.98949(6) 0.7500 0.29217(4) 0.00824(9) Uani 1 2 d S
Si7 Si 0.04027(2) 0.7500 0.078058(14) 0.00591(4) Uani 1 2 d S
O71 O 0.06901(4) 0.53259(7) 0.13704(3) 0.00885(7) Uani 1 1 d .
O72 O 0.13293(6) 0.7500 0.01421(4) 0.00855(10) Uani 1 2 d S
O73 O -0.09131(5) 0.7500 0.02952(4) 0.00907(10) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O62 Li1 O63 80.86(6) 1_455 1_455
O62 Li1 O33 100.19(7) 1_455 .
O63 Li1 O33 178.22(15) 1_455 .
O62 Li1 O32 177.61(18) 1_455 .
O63 Li1 O32 98.32(7) 1_455 .
O33 Li1 O32 80.57(6) . .
O62 Li1 Si6 40.73(3) 1_455 1_455
O63 Li1 Si6 40.53(3) 1_455 1_455
O33 Li1 Si6 140.67(8) . 1_455
O32 Li1 Si6 138.67(8) . 1_455
O62 Li1 Si3 139.99(8) 1_455 .
O63 Li1 Si3 138.34(8) 1_455 .
O33 Li1 Si3 40.40(3) . .
O32 Li1 Si3 40.48(3) . .
Si6 Li1 Si3 177.90(14) 1_455 .
O62 Li1 O43 95.31(10) 1_455 3_666
O63 Li1 O43 96.32(10) 1_455 3_666
O33 Li1 O43 85.03(9) . 3_666
O32 Li1 O43 87.01(10) . 3_666
Si6 Li1 O43 93.25(8) 1_455 3_666
Si3 Li1 O43 88.65(8) . 3_666
O62 Li1 O53 85.03(10) 1_455 1_455
O63 Li1 O53 83.20(9) 1_455 1_455
O33 Li1 O53 95.45(10) . 1_455
O32 Li1 O53 92.65(10) . 1_455
Si6 Li1 O53 86.65(8) 1_455 1_455
Si3 Li1 O53 91.44(8) . 1_455
O43 Li1 O53 179.36(7) 3_666 1_455
O62 Li1 Li9 85.92(8) 1_455 2_656
O63 Li1 Li9 135.62(13) 1_455 2_656
O33 Li1 Li9 46.05(6) . 2_656
O32 Li1 Li9 96.20(9) . 2_656
Si6 Li1 Li9 111.77(9) 1_455 2_656
Si3 Li1 Li9 70.27(6) . 2_656
O43 Li1 Li9 42.91(6) 3_666 2_656
O53 Li1 Li9 137.68(8) 1_455 2_656
O62 Li1 Li6 134.74(13) 1_455 3_666
O63 Li1 Li6 84.74(8) 1_455 3_666
O33 Li1 Li6 95.46(9) . 3_666
O32 Li1 Li6 47.19(6) . 3_666
Si6 Li1 Li6 110.35(8) 1_455 3_666
Si3 Li1 Li6 70.48(6) . 3_666
O43 Li1 Li6 44.04(6) 3_666 3_666
O53 Li1 Li6 135.44(9) 1_455 3_666
Li9 Li1 Li6 75.14(9) 2_656 3_666
O62 Li1 Li7 94.26(9) 1_455 .
O63 Li1 Li7 45.35(6) 1_455 .
O33 Li1 Li7 132.98(13) . .
O32 Li1 Li7 83.61(8) . .
Si6 Li1 Li7 68.90(6) 1_455 .
Si3 Li1 Li7 109.06(9) . .
O43 Li1 Li7 137.99(8) 3_666 .
O53 Li1 Li7 41.41(5) 1_455 .
Li9 Li1 Li7 179.02(10) 2_656 .
Li6 Li1 Li7 105.37(7) 3_666 .
O62 Li1 Li12 46.60(6) 1_455 1_455
O63 Li1 Li12 94.13(9) 1_455 1_455
O33 Li1 Li12 85.62(8) . 1_455
O32 Li1 Li12 131.42(13) . 1_455
Si6 Li1 Li12 69.64(6) 1_455 1_455
Si3 Li1 Li12 109.46(9) . 1_455
O43 Li1 Li12 137.95(9) 3_666 1_455
O53 Li1 Li12 42.57(6) 1_455 1_455
Li9 Li1 Li12 106.86(7) 2_656 1_455
Li6 Li1 Li12 177.90(11) 3_666 1_455
Li7 Li1 Li12 72.63(9) . 1_455
O31 Li2 O41 108.53(7) . 3_666
O31 Li2 O23 113.79(7) . .
O41 Li2 O23 116.35(6) 3_666 .
O31 Li2 O42 113.69(7) . .
O41 Li2 O42 101.94(6) 3_666 .
O23 Li2 O42 101.91(6) . .
O31 Li2 Li10 129.76(7) . 4_575
O41 Li2 Li10 120.88(7) 3_666 4_575
O23 Li2 Li10 51.90(4) . 4_575
O42 Li2 Li10 50.01(4) . 4_575
O31 Li2 Li8 129.30(7) . 3_666
O41 Li2 Li8 51.80(5) 3_666 3_666
O23 Li2 Li8 116.61(7) . 3_666
O42 Li2 Li8 50.41(5) . 3_666
Li10 Li2 Li8 80.66(7) 4_575 3_666
O31 Li2 Li4 79.68(5) . .
O41 Li2 Li4 105.08(6) 3_666 .
O23 Li2 Li4 44.14(4) . .
O42 Li2 Li4 143.87(7) . .
Li10 Li2 Li4 95.04(6) 4_575 .
Li8 Li2 Li4 144.99(6) 3_666 .
O31 Li2 Li6 87.97(6) . 3_666
O41 Li2 Li6 43.89(5) 3_666 3_666
O23 Li2 Li6 92.50(6) . 3_666
O42 Li2 Li6 145.37(6) . 3_666
Li10 Li2 Li6 134.07(7) 4_575 3_666
Li8 Li2 Li6 94.98(6) 3_666 3_666
Li4 Li2 Li6 63.24(5) . 3_666
O31 Li2 Li8 40.78(4) . .
O41 Li2 Li8 85.61(5) 3_666 .
O23 Li2 Li8 153.28(6) . .
O42 Li2 Li8 87.03(6) . .
Li10 Li2 Li8 131.15(7) 4_575 .
Li8 Li2 Li8 88.59(5) 3_666 .
Li4 Li2 Li8 118.34(6) . .
Li6 Li2 Li8 94.07(6) 3_666 .
O31 Li2 Si4 82.86(5) . .
O41 Li2 Si4 112.48(6) 3_666 .
O23 Li2 Si4 117.89(6) . .
O42 Li2 Si4 30.86(2) . .
Li10 Li2 Si4 71.11(5) 4_575 .
Li8 Li2 Si4 69.48(4) 3_666 .
Li4 Li2 Si4 141.95(5) . .
Li6 Li2 Si4 149.44(6) 3_666 .
Li8 Li2 Si4 60.55(4) . .
O31 Li2 Li2 38.29(4) . 4_565
O41 Li2 Li2 143.40(4) 3_666 4_565
O23 Li2 Li2 96.18(4) . 4_565
O42 Li2 Li2 86.19(4) . 4_565
Li10 Li2 Li2 91.82(4) 4_575 4_565
Li8 Li2 Li2 128.41(4) 3_666 4_565
Li4 Li2 Li2 86.23(4) . 4_565
Li6 Li2 Li2 123.70(3) 3_666 4_565
Li8 Li2 Li2 58.94(3) . 4_565
Si4 Li2 Li2 59.94(2) . 4_565
O31 Li2 Si3 27.68(3) . .
O41 Li2 Si3 95.66(5) 3_666 .
O23 Li2 Si3 100.54(5) . .
O42 Li2 Si3 141.35(6) . .
Li10 Li2 Si3 140.50(6) 4_575 .
Li8 Li2 Si3 138.17(7) 3_666 .
Li4 Li2 Si3 58.46(4) . .
Li6 Li2 Si3 63.35(4) 3_666 .
Li8 Li2 Si3 60.13(4) . .
Si4 Li2 Si3 110.49(4) . .
Li2 Li2 Si3 60.36(2) 4_565 .
O61 Li3 O52 109.61(6) . 4_575
O61 Li3 O52 109.61(6) . .
O52 Li3 O52 117.93(9) 4_575 .
O61 Li3 O21 118.13(9) . .
O52 Li3 O21 100.77(6) 4_575 .
O52 Li3 O21 100.77(6) . .
O61 Li3 Li5 134.04(6) . 4_575
O52 Li3 Li5 52.62(4) 4_575 4_575
O52 Li3 Li5 115.99(8) . 4_575
O21 Li3 Li5 48.46(5) . 4_575
O61 Li3 Li5 134.04(6) . .
O52 Li3 Li5 115.99(8) 4_575 .
O52 Li3 Li5 52.62(4) . .
O21 Li3 Li5 48.46(5) . .
Li5 Li3 Li5 75.18(8) 4_575 .
O61 Li3 Li10 41.81(4) . 4_575
O52 Li3 Li10 149.21(7) 4_575 4_575
O52 Li3 Li10 88.15(4) . 4_575
O21 Li3 Li10 89.07(6) . 4_575
Li5 Li3 Li10 132.60(8) 4_575 4_575
Li5 Li3 Li10 92.42(5) . 4_575
O61 Li3 Li10 41.81(4) . .
O52 Li3 Li10 88.15(4) 4_575 .
O52 Li3 Li10 149.21(7) . .
O21 Li3 Li10 89.07(6) . .
Li5 Li3 Li10 92.42(5) 4_575 .
Li5 Li3 Li10 132.60(8) . .
Li10 Li3 Li10 62.68(6) 4_575 .
O61 Li3 Li7 85.01(7) . 4_675
O52 Li3 Li7 44.30(4) 4_575 4_675
O52 Li3 Li7 94.91(7) . 4_675
O21 Li3 Li7 144.77(6) . 4_675
Li5 Li3 Li7 96.31(5) 4_575 4_675
Li5 Li3 Li7 132.87(8) . 4_675
Li10 Li3 Li7 123.03(7) 4_575 4_675
Li10 Li3 Li7 93.36(5) . 4_675
O61 Li3 Li7 85.01(7) . 1_655
O52 Li3 Li7 94.91(7) 4_575 1_655
O52 Li3 Li7 44.30(4) . 1_655
O21 Li3 Li7 144.77(6) . 1_655
Li5 Li3 Li7 132.87(8) 4_575 1_655
Li5 Li3 Li7 96.31(5) . 1_655
Li10 Li3 Li7 93.36(5) 4_575 1_655
Li10 Li3 Li7 123.03(7) . 1_655
Li7 Li3 Li7 55.75(6) 4_675 1_655
O61 Li3 Si2 86.50(7) . .
O52 Li3 Si2 114.28(6) 4_575 .
O52 Li3 Si2 114.28(6) . .
O21 Li3 Si2 31.63(3) . .
Li5 Li3 Si2 70.29(5) 4_575 .
Li5 Li3 Si2 70.29(5) . .
Li10 Li3 Si2 62.51(4) 4_575 .
Li10 Li3 Si2 62.51(4) . .
Li7 Li3 Si2 150.78(4) 4_675 .
Li7 Li3 Si2 150.78(4) 1_655 .
O61 Li3 Si6 27.48(4) . .
O52 Li3 Si6 96.73(6) 4_575 .
O52 Li3 Si6 96.73(6) . .
O21 Li3 Si6 145.61(8) . .
Li5 Li3 Si6 142.39(4) 4_575 .
Li5 Li3 Si6 142.39(4) . .
Li10 Li3 Si6 62.03(4) 4_575 .
Li10 Li3 Si6 62.03(4) . .
Li7 Li3 Si6 61.11(5) 4_675 .
Li7 Li3 Si6 61.11(5) 1_655 .
Si2 Li3 Si6 113.98(6) . .
O23 Li4 O13 114.67(7) . .
O23 Li4 O32 124.06(7) . .
O13 Li4 O32 113.49(7) . .
O23 Li4 O22 84.35(5) . .
O13 Li4 O22 104.39(6) . .
O32 Li4 O22 109.38(6) . .
O23 Li4 Li14 122.70(7) . .
O13 Li4 Li14 54.93(5) . .
O32 Li4 Li14 107.55(7) . .
O22 Li4 Li14 54.24(5) . .
O23 Li4 Si2 41.66(3) . .
O13 Li4 Si2 114.90(6) . .
O32 Li4 Si2 128.95(6) . .
O22 Li4 Si2 42.76(3) . .
Li14 Li4 Si2 87.72(5) . .
O23 Li4 Li4 101.75(4) . 4_565
O13 Li4 Li4 47.56(4) . 4_565
O32 Li4 Li4 90.45(4) . 4_565
O22 Li4 Li4 151.42(4) . 4_565
Li14 Li4 Li4 100.92(5) . 4_565
Si2 Li4 Li4 135.19(3) . 4_565
O23 Li4 Li19 160.66(7) . 1_455
O13 Li4 Li19 61.21(7) . 1_455
O32 Li4 Li19 52.87(7) . 1_455
O22 Li4 Li19 114.94(7) . 1_455
Li14 Li4 Li19 71.95(7) . 1_455
Si2 Li4 Li19 157.46(7) . 1_455
Li4 Li4 Li19 60.85(4) 4_565 1_455
O23 Li4 Li2 44.93(4) . .
O13 Li4 Li2 136.44(7) . .
O32 Li4 Li2 80.32(5) . .
O22 Li4 Li2 109.34(6) . .
Li14 Li4 Li2 163.15(7) . .
Si2 Li4 Li2 75.97(4) . .
Li4 Li4 Li2 93.77(4) 4_565 .
Li19 Li4 Li2 123.19(8) 1_455 .
O23 Li4 Li13 127.03(7) . .
O13 Li4 Li13 111.96(7) . .
O32 Li4 Li13 50.66(5) . .
O22 Li4 Li13 60.66(5) . .
Li14 Li4 Li13 68.65(6) . .
Si2 Li4 Li13 95.88(5) . .
Li4 Li4 Li13 128.37(4) 4_565 .
Li19 Li4 Li13 68.07(5) 1_455 .
Li2 Li4 Li13 108.30(6) . .
O23 Li4 Li11 45.07(4) . .
O13 Li4 Li11 71.97(5) . .
O32 Li4 Li11 138.51(7) . .
O22 Li4 Li11 108.50(6) . .
Li14 Li4 Li11 107.92(6) . .
Si2 Li4 Li11 73.20(4) . .
Li4 Li4 Li11 62.25(3) 4_565 .
Li19 Li4 Li11 121.69(6) 1_455 .
Li2 Li4 Li11 71.73(5) . .
Li13 Li4 Li11 168.86(6) . .
O23 Li4 Si3 107.61(5) . .
O13 Li4 Si3 102.34(5) . .
O32 Li4 Si3 34.52(2) . .
O22 Li4 Si3 142.52(6) . .
Li14 Li4 Si3 129.55(6) . .
Si2 Li4 Si3 138.95(5) . .
Li4 Li4 Si3 62.52(3) 4_565 .
Li19 Li4 Si3 58.20(6) 1_455 .
Li2 Li4 Si3 64.98(4) . .
Li13 Li4 Si3 85.15(5) . .
Li11 Li4 Si3 104.46(5) . .
O11 Li5 O21 109.90(6) . .
O11 Li5 O12 113.16(7) . 3_665
O21 Li5 O12 117.92(6) . 3_665
O11 Li5 O52 113.22(6) . .
O21 Li5 O52 102.81(6) . .
O12 Li5 O52 98.91(6) 3_665 .
O11 Li5 Li16 127.06(7) . 4_565
O21 Li5 Li16 122.04(7) . 4_565
O12 Li5 Li16 50.62(4) 3_665 4_565
O52 Li5 Li16 48.29(4) . 4_565
O11 Li5 Li3 130.89(7) . .
O21 Li5 Li3 53.44(5) . .
O12 Li5 Li3 114.90(7) 3_665 .
O52 Li5 Li3 49.69(4) . .
Li16 Li5 Li3 79.32(6) 4_565 .
O11 Li5 Li17 69.19(6) . 3_665
O21 Li5 Li17 141.48(7) . 3_665
O12 Li5 Li17 44.21(5) 3_665 3_665
O52 Li5 Li17 112.91(7) . 3_665
Li16 Li5 Li17 76.15(7) 4_565 3_665
Li3 Li5 Li17 155.20(8) . 3_665
O11 Li5 Li17 90.75(6) . .
O21 Li5 Li17 47.63(5) . .
O12 Li5 Li17 89.30(7) 3_665 .
O52 Li5 Li17 148.46(6) . .
Li16 Li5 Li17 131.26(7) 4_565 .
Li3 Li5 Li17 99.26(6) . .
Li17 Li5 Li17 94.21(6) 3_665 .
O11 Li5 Li11 42.59(4) . .
O21 Li5 Li11 85.99(5) . .
O12 Li5 Li11 153.32(6) 3_665 .
O52 Li5 Li11 85.97(6) . .
Li16 Li5 Li11 128.21(7) 4_565 .
Li3 Li5 Li11 88.30(6) . .
Li17 Li5 Li11 109.76(6) 3_665 .
Li17 Li5 Li11 100.22(7) . .
O11 Li5 Li5 36.63(4) . 4_565
O21 Li5 Li5 142.90(4) . 4_565
O12 Li5 Li5 95.64(4) 3_665 4_565
O52 Li5 Li5 85.86(4) . 4_565
Li16 Li5 Li5 90.81(4) 4_565 4_565
Li3 Li5 Li5 127.59(4) . 4_565
Li17 Li5 Li5 56.84(4) 3_665 4_565
Li17 Li5 Li5 123.81(4) . 4_565
Li11 Li5 Li5 58.36(3) . 4_565
O11 Li5 Si5 83.31(5) . .
O21 Li5 Si5 112.90(6) . .
O12 Li5 Si5 114.54(5) 3_665 .
O52 Li5 Si5 30.00(2) . .
Li16 Li5 Si5 68.58(4) 4_565 .
Li3 Li5 Si5 68.34(4) . .
Li17 Li5 Si5 105.31(5) 3_665 .
Li17 Li5 Si5 155.89(7) . .
Li11 Li5 Si5 60.16(4) . .
Li5 Li5 Si5 60.26(2) 4_565 .
O11 Li5 Si1 27.05(3) . .
O21 Li5 Si1 94.00(5) . .
O12 Li5 Si1 104.95(5) 3_665 .
O52 Li5 Si1 139.84(5) . .
Li16 Li5 Si1 142.26(6) 4_565 .
Li3 Li5 Si1 136.87(6) . .
Li17 Li5 Si1 67.89(5) 3_665 .
Li17 Li5 Si1 64.37(4) . .
Li11 Li5 Si1 58.84(4) . .
Li5 Li5 Si1 60.30(2) 4_565 .
Si5 Li5 Si1 109.84(4) . .
O41 Li6 O43 84.09(8) . .
O41 Li6 O32 119.25(6) . 3_666
O43 Li6 O32 104.63(7) . 3_666
O41 Li6 O32 119.25(6) . 2_646
O43 Li6 O32 104.63(7) . 2_646
O32 Li6 O32 116.09(9) 3_666 2_646
O41 Li6 Li13 157.10(12) . 3_666
O43 Li6 Li13 118.82(11) . 3_666
O32 Li6 Li13 58.04(5) 3_666 3_666
O32 Li6 Li13 58.04(5) 2_646 3_666
O41 Li6 Si4 41.42(4) . .
O43 Li6 Si4 42.66(4) . .
O32 Li6 Si4 120.06(5) 3_666 .
O32 Li6 Si4 120.06(5) 2_646 .
Li13 Li6 Si4 161.48(11) 3_666 .
O41 Li6 Li1 130.48(8) . 3_666
O43 Li6 Li1 62.61(7) . 3_666
O32 Li6 Li1 47.72(6) 3_666 3_666
O32 Li6 Li1 104.69(9) 2_646 3_666
Li13 Li6 Li1 66.93(8) 3_666 3_666
Si4 Li6 Li1 97.84(8) . 3_666
O41 Li6 Li1 130.48(8) . 2_646
O43 Li6 Li1 62.61(7) . 2_646
O32 Li6 Li1 104.69(9) 3_666 2_646
O32 Li6 Li1 47.72(6) 2_646 2_646
Li13 Li6 Li1 66.93(8) 3_666 2_646
Si4 Li6 Li1 97.84(8) . 2_646
Li1 Li6 Li1 66.18(8) 3_666 2_646
O41 Li6 Li2 43.67(4) . 2_646
O43 Li6 Li2 109.53(7) . 2_646
O32 Li6 Li2 137.79(9) 3_666 2_646
O32 Li6 Li2 78.41(5) 2_646 2_646
Li13 Li6 Li2 120.42(8) 3_666 2_646
Si4 Li6 Li2 74.31(5) . 2_646
Li1 Li6 Li2 171.96(10) 3_666 2_646
Li1 Li6 Li2 112.61(4) 2_646 2_646
O41 Li6 Li2 43.67(4) . 3_666
O43 Li6 Li2 109.53(7) . 3_666
O32 Li6 Li2 78.41(5) 3_666 3_666
O32 Li6 Li2 137.79(9) 2_646 3_666
Li13 Li6 Li2 120.42(8) 3_666 3_666
Si4 Li6 Li2 74.31(5) . 3_666
Li1 Li6 Li2 112.61(4) 3_666 3_666
Li1 Li6 Li2 171.96(10) 2_646 3_666
Li2 Li6 Li2 67.40(7) 2_646 3_666
O41 Li6 Li4 99.69(8) . 3_666
O43 Li6 Li4 143.10(4) . 3_666
O32 Li6 Li4 41.73(4) 3_666 3_666
O32 Li6 Li4 105.18(8) 2_646 3_666
Li13 Li6 Li4 62.54(6) 3_666 3_666
Si4 Li6 Li4 130.29(6) . 3_666
Li1 Li6 Li4 89.03(6) 3_666 3_666
Li1 Li6 Li4 129.18(9) 2_646 3_666
Li2 Li6 Li4 97.36(7) 2_646 3_666
Li2 Li6 Li4 57.91(5) 3_666 3_666
O41 Li6 Li4 99.69(8) . 2_646
O43 Li6 Li4 143.10(4) . 2_646
O32 Li6 Li4 105.18(8) 3_666 2_646
O32 Li6 Li4 41.73(4) 2_646 2_646
Li13 Li6 Li4 62.54(6) 3_666 2_646
Si4 Li6 Li4 130.29(6) . 2_646
Li1 Li6 Li4 129.18(9) 3_666 2_646
Li1 Li6 Li4 89.03(6) 2_646 2_646
Li2 Li6 Li4 57.91(5) 2_646 2_646
Li2 Li6 Li4 97.36(7) 3_666 2_646
Li4 Li6 Li4 72.90(7) 3_666 2_646
O53 Li7 O71 111.52(7) 1_455 .
O53 Li7 O63 108.25(7) 1_455 1_455
O71 Li7 O63 108.95(7) . 1_455
O53 Li7 O52 84.58(5) 1_455 1_455
O71 Li7 O52 117.99(7) . 1_455
O63 Li7 O52 122.21(7) 1_455 1_455
O53 Li7 Si5 43.14(3) 1_455 1_455
O71 Li7 Si5 126.22(6) . 1_455
O63 Li7 Si5 123.33(6) 1_455 1_455
O52 Li7 Si5 41.50(3) 1_455 1_455
O53 Li7 Li13 120.12(8) 1_455 .
O71 Li7 Li13 54.35(6) . .
O63 Li7 Li13 55.01(6) 1_455 .
O52 Li7 Li13 155.24(8) 1_455 .
Si5 Li7 Li13 163.25(7) 1_455 .
O53 Li7 Li7 153.28(4) 1_455 4_575
O71 Li7 Li7 89.65(4) . 4_575
O63 Li7 Li7 47.16(4) 1_455 4_575
O52 Li7 Li7 100.12(4) 1_455 4_575
Si5 Li7 Li7 134.52(3) 1_455 4_575
Li13 Li7 Li7 58.92(4) . 4_575
O53 Li7 Li19 61.52(7) 1_455 1_455
O71 Li7 Li19 52.78(7) . 1_455
O63 Li7 Li19 109.09(8) 1_455 1_455
O52 Li7 Li19 125.42(7) 1_455 1_455
Si5 Li7 Li19 95.71(6) 1_455 1_455
Li13 Li7 Li19 71.39(6) . 1_455
Li7 Li7 Li19 129.73(5) 4_575 1_455
O53 Li7 Li1 66.13(7) 1_455 .
O71 Li7 Li1 104.73(7) . .
O63 Li7 Li1 47.59(6) 1_455 .
O52 Li7 Li1 134.94(7) 1_455 .
Si5 Li7 Li1 101.51(7) 1_455 .
Li13 Li7 Li1 64.54(7) . .
Li7 Li7 Li1 93.51(6) 4_575 .
Li19 Li7 Li1 70.24(7) 1_455 .
O53 Li7 Si7 143.12(6) 1_455 .
O71 Li7 Si7 33.90(3) . .
O63 Li7 Si7 99.11(5) 1_455 .
O52 Li7 Si7 101.51(5) 1_455 .
Si5 Li7 Si7 133.37(5) 1_455 .
Li13 Li7 Si7 58.37(5) . .
Li7 Li7 Si7 62.12(3) 4_575 .
Li19 Li7 Si7 86.66(7) 1_455 .
Li1 Li7 Si7 122.64(7) . .
O53 Li7 Li3 108.84(6) 1_455 1_455
O71 Li7 Li3 132.63(7) . 1_455
O63 Li7 Li3 80.12(5) 1_455 1_455
O52 Li7 Li3 43.51(4) 1_455 1_455
Si5 Li7 Li3 72.54(4) 1_455 1_455
Li13 Li7 Li3 120.59(6) . 1_455
Li7 Li7 Li3 62.13(3) 4_575 1_455
Li19 Li7 Li3 168.02(7) 1_455 1_455
Li1 Li7 Li3 113.64(7) . 1_455
Si7 Li7 Li3 99.67(5) . 1_455
O53 Li7 Li16 106.62(6) 1_455 4_465
O71 Li7 Li16 77.74(5) . 4_465
O63 Li7 Li16 138.47(7) 1_455 4_465
O52 Li7 Li16 40.95(4) 1_455 4_465
Si5 Li7 Li16 71.86(4) 1_455 4_465
Li13 Li7 Li16 121.44(7) . 4_465
Li7 Li7 Li16 93.33(4) 4_575 4_465
Li19 Li7 Li16 106.96(7) 1_455 4_465
Li1 Li7 Li16 172.75(8) . 4_465
Si7 Li7 Li16 63.08(4) . 4_465
Li3 Li7 Li16 67.73(5) 1_455 4_465
O31 Li8 O42 111.28(6) . 3_666
O31 Li8 O42 111.28(6) . 2_646
O42 Li8 O42 117.86(9) 3_666 2_646
O31 Li8 O41 114.58(9) . .
O42 Li8 O41 100.53(6) 3_666 .
O42 Li8 O41 100.53(6) 2_646 .
O31 Li8 Li2 131.87(6) . 3_666
O42 Li8 Li2 51.40(4) 3_666 3_666
O42 Li8 Li2 116.13(9) 2_646 3_666
O41 Li8 Li2 49.40(5) . 3_666
O31 Li8 Li2 131.87(6) . 2_646
O42 Li8 Li2 116.13(9) 3_666 2_646
O42 Li8 Li2 51.40(4) 2_646 2_646
O41 Li8 Li2 49.40(5) . 2_646
Li2 Li8 Li2 76.83(8) 3_666 2_646
O31 Li8 Li9 88.31(7) . 3_656
O42 Li8 Li9 94.99(7) 3_666 3_656
O42 Li8 Li9 44.45(5) 2_646 3_656
O41 Li8 Li9 144.66(6) . 3_656
Li2 Li8 Li9 132.28(8) 3_666 3_656
Li2 Li8 Li9 95.26(5) 2_646 3_656
O31 Li8 Li9 88.31(7) . 2_656
O42 Li8 Li9 44.45(4) 3_666 2_656
O42 Li8 Li9 94.99(7) 2_646 2_656
O41 Li8 Li9 144.66(6) . 2_656
Li2 Li8 Li9 95.26(5) 3_666 2_656
Li2 Li8 Li9 132.28(8) 2_646 2_656
Li9 Li8 Li9 55.75(6) 3_656 2_656
O31 Li8 Li2 40.53(4) . 4_565
O42 Li8 Li2 149.63(7) 3_666 4_565
O42 Li8 Li2 88.79(4) 2_646 4_565
O41 Li8 Li2 87.53(6) . 4_565
Li2 Li8 Li2 131.75(7) 3_666 4_565
Li2 Li8 Li2 91.41(5) 2_646 4_565
Li9 Li8 Li2 94.89(5) 3_656 4_565
Li9 Li8 Li2 124.60(7) 2_656 4_565
O31 Li8 Li2 40.53(4) . .
O42 Li8 Li2 88.79(4) 3_666 .
O42 Li8 Li2 149.63(7) 2_646 .
O41 Li8 Li2 87.53(6) . .
Li2 Li8 Li2 91.41(5) 3_666 .
Li2 Li8 Li2 131.75(7) 2_646 .
Li9 Li8 Li2 124.60(7) 3_656 .
Li9 Li8 Li2 94.89(5) 2_656 .
Li2 Li8 Li2 62.13(6) 4_565 .
O31 Li8 Si4 83.21(6) . .
O42 Li8 Si4 114.03(5) 3_666 .
O42 Li8 Si4 114.03(5) 2_646 .
O41 Li8 Si4 31.37(3) . .
Li2 Li8 Si4 70.82(5) 3_666 .
Li2 Li8 Si4 70.82(5) 2_646 .
Li9 Li8 Si4 150.90(4) 3_656 .
Li9 Li8 Si4 150.90(4) 2_656 .
Li2 Li8 Si4 61.18(4) 4_565 .
Li2 Li8 Si4 61.18(4) . .
O31 Li8 Si3 29.34(4) . .
O42 Li8 Si3 97.85(6) 3_666 .
O42 Li8 Si3 97.85(6) 2_646 .
O41 Li8 Si3 143.92(8) . .
Li2 Li8 Si3 141.53(4) 3_666 .
Li2 Li8 Si3 141.53(4) 2_646 .
Li9 Li8 Si3 62.70(5) 3_656 .
Li9 Li8 Si3 62.70(5) 2_656 .
Li2 Li8 Si3 62.03(4) 4_565 .
Li2 Li8 Si3 62.03(4) . .
Si4 Li8 Si3 112.55(6) . .
O43 Li9 O62 111.62(7) . 4_565
O43 Li9 O33 107.40(7) . 3_656
O62 Li9 O33 110.66(7) 4_565 3_656
O43 Li9 O42 84.23(6) . 4_565
O62 Li9 O42 118.91(7) 4_565 4_565
O33 Li9 O42 120.01(7) 3_656 4_565
O43 Li9 Si4 42.93(3) . .
O62 Li9 Si4 126.67(6) 4_565 .
O33 Li9 Si4 121.20(6) 3_656 .
O42 Li9 Si4 41.35(3) 4_565 .
O43 Li9 Li18 119.27(8) . 3_656
O62 Li9 Li18 54.36(7) 4_565 3_656
O33 Li9 Li18 56.84(7) 3_656 3_656
O42 Li9 Li18 156.48(8) 4_565 3_656
Si4 Li9 Li18 162.17(7) . 3_656
O43 Li9 Li9 152.83(4) . 4
O62 Li9 Li9 89.76(4) 4_565 4
O33 Li9 Li9 47.15(4) 3_656 4
O42 Li9 Li9 100.37(4) 4_565 4
Si4 Li9 Li9 134.52(3) . 4
Li18 Li9 Li9 59.46(4) 3_656 4
O43 Li9 Li1 64.39(7) . 2_646
O62 Li9 Li1 105.79(7) 4_565 2_646
O33 Li9 Li1 48.82(6) 3_656 2_646
O42 Li9 Li1 132.59(7) 4_565 2_646
Si4 Li9 Li1 99.29(7) . 2_646
Li18 Li9 Li1 65.63(8) 3_656 2_646
Li9 Li9 Li1 94.48(6) 4 2_646
O43 Li9 Li18 62.16(6) . 1_655
O62 Li9 Li18 52.51(6) 4_565 1_655
O33 Li9 Li18 109.41(8) 3_656 1_655
O42 Li9 Li18 126.71(7) 4_565 1_655
Si4 Li9 Li18 96.62(6) . 1_655
Li18 Li9 Li18 69.81(4) 3_656 1_655
Li9 Li9 Li18 128.74(5) 4 1_655
Li1 Li9 Li18 69.67(7) 2_646 1_655
O43 Li9 Li8 108.34(6) . 3_656
O62 Li9 Li8 133.65(7) 4_565 3_656
O33 Li9 Li8 77.77(5) 3_656 3_656
O42 Li9 Li8 43.85(4) 4_565 3_656
Si4 Li9 Li8 72.53(4) . 3_656
Li18 Li9 Li8 120.93(6) 3_656 3_656
Li9 Li9 Li8 62.12(3) 4 3_656
Li1 Li9 Li8 112.06(7) 2_646 3_656
Li18 Li9 Li8 169.13(7) 1_655 3_656
O43 Li9 Si6 143.31(6) . 1_545
O62 Li9 Si6 33.96(3) 4_565 1_545
O33 Li9 Si6 100.37(5) 3_656 1_545
O42 Li9 Si6 102.31(6) 4_565 1_545
Si4 Li9 Si6 133.92(6) . 1_545
Li18 Li9 Si6 58.91(6) 3_656 1_545
Li9 Li9 Si6 62.30(3) 4 1_545
Li1 Li9 Si6 124.29(7) 2_646 1_545
Li18 Li9 Si6 86.43(6) 1_655 1_545
Li8 Li9 Si6 100.51(5) 3_656 1_545
O43 Li9 Li10 107.30(6) . 1_545
O62 Li9 Li10 78.41(5) 4_565 1_545
O33 Li9 Li10 137.14(7) 3_656 1_545
O42 Li9 Li10 41.38(4) 4_565 1_545
Si4 Li9 Li10 72.47(4) . 1_545
Li18 Li9 Li10 122.08(7) 3_656 1_545
Li9 Li9 Li10 92.89(4) 4 1_545
Li1 Li9 Li10 171.52(8) 2_646 1_545
Li18 Li9 Li10 108.63(7) 1_655 1_545
Li8 Li9 Li10 67.98(5) 3_656 1_545
Si6 Li9 Li10 63.19(4) 1_545 1_545
O61 Li10 O51 109.73(7) . 1_565
O61 Li10 O42 112.08(7) . 4_575
O51 Li10 O42 114.55(7) 1_565 4_575
O61 Li10 O23 115.48(7) . 4_575
O51 Li10 O23 101.92(6) 1_565 4_575
O42 Li10 O23 102.67(6) 4_575 4_575
O61 Li10 Li2 130.16(7) . 4_575
O51 Li10 Li2 119.78(7) 1_565 4_575
O42 Li10 Li2 52.08(5) 4_575 4_575
O23 Li10 Li2 50.59(4) 4_575 4_575
O61 Li10 Li11 130.40(7) . 1_565
O51 Li10 Li11 52.09(5) 1_565 1_565
O42 Li10 Li11 117.36(7) 4_575 1_565
O23 Li10 Li11 49.94(5) 4_575 1_565
Li2 Li10 Li11 81.03(7) 4_575 1_565
O61 Li10 Li12 87.44(6) . 1_565
O51 Li10 Li12 44.77(5) 1_565 1_565
O42 Li10 Li12 89.94(6) 4_575 1_565
O23 Li10 Li12 146.09(7) 4_575 1_565
Li2 Li10 Li12 132.11(7) 4_575 1_565
Li11 Li10 Li12 96.27(6) 1_565 1_565
O61 Li10 Li3 42.22(4) . .
O51 Li10 Li3 87.53(5) 1_565 .
O42 Li10 Li3 152.86(7) 4_575 .
O23 Li10 Li3 86.89(6) 4_575 .
Li2 Li10 Li3 131.35(7) 4_575 .
Li11 Li10 Li3 88.34(6) 1_565 .
Li12 Li10 Li3 96.06(6) 1_565 .
O61 Li10 Li9 78.90(5) . 1_565
O51 Li10 Li9 103.97(6) 1_565 1_565
O42 Li10 Li9 42.72(4) 4_575 1_565
O23 Li10 Li9 143.54(6) 4_575 1_565
Li2 Li10 Li9 93.92(6) 4_575 1_565
Li11 Li10 Li9 144.61(6) 1_565 1_565
Li12 Li10 Li9 61.51(5) 1_565 1_565
Li3 Li10 Li9 119.29(6) . 1_565
O61 Li10 Li10 39.10(4) . 4_575
O51 Li10 Li10 145.00(4) 1_565 4_575
O42 Li10 Li10 96.25(4) 4_575 4_575
O23 Li10 Li10 86.19(4) 4_575 4_575
Li2 Li10 Li10 91.82(5) 4_575 4_575
Li11 Li10 Li10 127.83(4) 1_565 4_575
Li12 Li10 Li10 124.04(4) 1_565 4_575
Li3 Li10 Li10 58.66(3) . 4_575
Li9 Li10 Li10 87.11(3) 1_565 4_575
O61 Li10 Si2 85.43(5) . .
O51 Li10 Si2 112.87(6) 1_565 .
O42 Li10 Si2 118.43(6) 4_575 .
O23 Li10 Si2 30.10(2) 4_575 .
Li2 Li10 Si2 71.17(5) 4_575 .
Li11 Li10 Si2 68.22(4) 1_565 .
Li12 Li10 Si2 151.34(6) 1_565 .
Li3 Li10 Si2 60.86(4) . .
Li9 Li10 Si2 143.00(5) 1_565 .
Li10 Li10 Si2 60.68(2) 4_575 .
O61 Li10 Si6 27.27(3) . .
O51 Li10 Si6 97.08(5) 1_565 .
O42 Li10 Si6 98.00(5) 4_575 .
O23 Li10 Si6 142.75(6) 4_575 .
Li2 Li10 Si6 138.88(6) 4_575 .
Li11 Li10 Si6 139.68(6) 1_565 .
Li12 Li10 Si6 63.24(4) 1_565 .
Li3 Li10 Si6 62.09(4) . .
Li9 Li10 Si6 57.43(4) 1_565 .
Li10 Li10 Si6 60.82(2) 4_575 .
Si2 Li10 Si6 112.69(4) . .
O11 Li11 O23 113.22(6) . .
O11 Li11 O23 113.22(6) . 4_565
O23 Li11 O23 117.62(9) . 4_565
O11 Li11 O51 115.51(9) . .
O23 Li11 O51 97.65(6) . .
O23 Li11 O51 97.65(6) 4_565 .
O11 Li11 Li10 131.39(6) . 4_575
O23 Li11 Li10 50.18(4) . 4_575
O23 Li11 Li10 114.14(8) 4_565 4_575
O51 Li11 Li10 47.57(4) . 4_575
O11 Li11 Li10 131.39(6) . 1_545
O23 Li11 Li10 114.14(8) . 1_545
O23 Li11 Li10 50.18(4) 4_565 1_545
O51 Li11 Li10 47.57(4) . 1_545
Li10 Li11 Li10 75.65(8) 4_575 1_545
O11 Li11 Li4 94.60(7) . 4_565
O23 Li11 Li4 94.06(7) . 4_565
O23 Li11 Li4 43.46(4) 4_565 4_565
O51 Li11 Li4 139.54(6) . 4_565
Li10 Li11 Li4 127.83(8) 4_575 4_565
Li10 Li11 Li4 92.42(5) 1_545 4_565
O11 Li11 Li4 94.60(7) . .
O23 Li11 Li4 43.46(4) . .
O23 Li11 Li4 94.06(7) 4_565 .
O51 Li11 Li4 139.54(6) . .
Li10 Li11 Li4 92.42(5) 4_575 .
Li10 Li11 Li4 127.83(8) 1_545 .
Li4 Li11 Li4 55.50(6) 4_565 .
O11 Li11 Li5 40.46(4) . 4_565
O23 Li11 Li5 151.29(7) . 4_565
O23 Li11 Li5 88.82(4) 4_565 4_565
O51 Li11 Li5 89.02(6) . 4_565
Li10 Li11 Li5 131.29(8) 4_575 4_565
Li10 Li11 Li5 90.94(5) 1_545 4_565
Li4 Li11 Li5 98.82(5) 4_565 4_565
Li4 Li11 Li5 129.94(8) . 4_565
O11 Li11 Li5 40.46(4) . .
O23 Li11 Li5 88.82(4) . .
O23 Li11 Li5 151.29(7) 4_565 .
O51 Li11 Li5 89.02(6) . .
Li10 Li11 Li5 90.94(5) 4_575 .
Li10 Li11 Li5 131.29(8) 1_545 .
Li4 Li11 Li5 129.94(8) 4_565 .
Li4 Li11 Li5 98.82(5) . .
Li5 Li11 Li5 63.29(6) 4_565 .
O11 Li11 Si1 31.71(4) . .
O23 Li11 Si1 99.15(6) . .
O23 Li11 Si1 99.15(6) 4_565 .
O51 Li11 Si1 147.22(8) . .
Li10 Li11 Si1 142.15(4) 4_575 .
Li10 Li11 Si1 142.15(4) 1_545 .
Li4 Li11 Si1 66.74(5) 4_565 .
Li4 Li11 Si1 66.74(5) . .
Li5 Li11 Si1 63.48(4) 4_565 .
Li5 Li11 Si1 63.48(4) . .
O11 Li11 Si5 84.04(6) . .
O23 Li11 Si5 112.02(6) . .
O23 Li11 Si5 112.02(6) 4_565 .
O51 Li11 Si5 31.47(3) . .
Li10 Li11 Si5 68.84(5) 4_575 .
Li10 Li11 Si5 68.84(5) 1_545 .
Li4 Li11 Si5 152.24(3) 4_565 .
Li4 Li11 Si5 152.24(3) . .
Li5 Li11 Si5 62.68(4) 4_565 .
Li5 Li11 Si5 62.68(4) . .
Si1 Li11 Si5 115.75(6) . .
O51 Li12 O53 83.40(8) . .
O51 Li12 O62 120.33(6) . .
O53 Li12 O62 104.57(7) . .
O51 Li12 O62 120.33(6) . 4_565
O53 Li12 O62 104.57(7) . 4_565
O62 Li12 O62 114.46(10) . 4_565
O51 Li12 Li18 157.41(13) . 1_655
O53 Li12 Li18 119.19(12) . 1_655
O62 Li12 Li18 57.24(5) . 1_655
O62 Li12 Li18 57.24(5) 4_565 1_655
O51 Li12 Si5 40.97(4) . .
O53 Li12 Si5 42.43(4) . .
O62 Li12 Si5 120.60(5) . .
O62 Li12 Si5 120.60(5) 4_565 .
Li18 Li12 Si5 161.62(12) 1_655 .
O51 Li12 Li10 43.07(4) . 1_545
O53 Li12 Li10 107.73(7) . 1_545
O62 Li12 Li10 139.76(10) . 1_545
O62 Li12 Li10 79.74(5) 4_565 1_545
Li18 Li12 Li10 121.62(9) 1_655 1_545
Si5 Li12 Li10 72.83(6) . 1_545
O51 Li12 Li10 43.07(4) . 4_575
O53 Li12 Li10 107.73(7) . 4_575
O62 Li12 Li10 79.74(5) . 4_575
O62 Li12 Li10 139.76(10) 4_565 4_575
Li18 Li12 Li10 121.62(9) 1_655 4_575
Si5 Li12 Li10 72.83(6) . 4_575
Li10 Li12 Li10 68.08(7) 1_545 4_575
O51 Li12 Li1 131.23(8) . 1_655
O53 Li12 Li1 64.06(7) . 1_655
O62 Li12 Li1 46.24(6) . 1_655
O62 Li12 Li1 103.15(9) 4_565 1_655
Li18 Li12 Li1 65.79(8) 1_655 1_655
Si5 Li12 Li1 99.14(8) . 1_655
Li10 Li12 Li1 171.68(10) 1_545 1_655
Li10 Li12 Li1 112.19(4) 4_575 1_655
O51 Li12 Li1 131.23(8) . 4_665
O53 Li12 Li1 64.06(7) . 4_665
O62 Li12 Li1 103.15(9) . 4_665
O62 Li12 Li1 46.24(6) 4_565 4_665
Li18 Li12 Li1 65.79(8) 1_655 4_665
Si5 Li12 Li1 99.14(8) . 4_665
Li10 Li12 Li1 112.19(4) 1_545 4_665
Li10 Li12 Li1 171.68(10) 4_575 4_665
Li1 Li12 Li1 66.26(8) 1_655 4_665
O51 Li12 Li9 102.08(8) . .
O53 Li12 Li9 143.29(4) . .
O62 Li12 Li9 103.57(8) . .
O62 Li12 Li9 41.33(4) 4_565 .
Li18 Li12 Li9 60.41(7) 1_655 .
Si5 Li12 Li9 132.16(6) . .
Li10 Li12 Li9 61.22(5) 1_545 .
Li10 Li12 Li9 100.06(8) 4_575 .
Li1 Li12 Li9 125.93(9) 1_655 .
Li1 Li12 Li9 86.92(6) 4_665 .
O51 Li12 Li9 102.08(8) . 4_565
O53 Li12 Li9 143.29(4) . 4_565
O62 Li12 Li9 41.33(4) . 4_565
O62 Li12 Li9 103.57(8) 4_565 4_565
Li18 Li12 Li9 60.41(7) 1_655 4_565
Si5 Li12 Li9 132.16(6) . 4_565
Li10 Li12 Li9 100.06(8) 1_545 4_565
Li10 Li12 Li9 61.22(5) 4_575 4_565
Li1 Li12 Li9 86.92(6) 1_655 4_565
Li1 Li12 Li9 125.93(9) 4_665 4_565
Li9 Li12 Li9 71.75(7) . 4_565
O71 Li13 O71 76.23(7) . 4_575
O71 Li13 O32 89.25(2) . .
O71 Li13 O32 164.90(8) 4_575 .
O71 Li13 O32 164.90(8) . 4_575
O71 Li13 O32 89.25(2) 4_575 4_575
O32 Li13 O32 104.89(9) . 4_575
O71 Li13 O63 94.52(8) . 1_455
O71 Li13 O63 94.52(8) 4_575 1_455
O32 Li13 O63 90.67(7) . 1_455
O32 Li13 O63 90.67(7) 4_575 1_455
O71 Li13 Li6 141.33(4) . 3_666
O71 Li13 Li6 141.33(4) 4_575 3_666
O32 Li13 Li6 52.44(5) . 3_666
O32 Li13 Li6 52.44(5) 4_575 3_666
O63 Li13 Li6 91.35(10) 1_455 3_666
O71 Li13 O22 89.70(8) . .
O71 Li13 O22 89.70(8) 4_575 .
O32 Li13 O22 86.07(7) . .
O32 Li13 O22 86.07(7) 4_575 .
O63 Li13 O22 174.64(11) 1_455 .
Li6 Li13 O22 83.29(9) 3_666 .
O71 Li13 Li7 47.06(5) . .
O71 Li13 Li7 87.48(8) 4_575 .
O32 Li13 Li7 85.53(5) . .
O32 Li13 Li7 137.78(11) 4_575 .
O63 Li13 Li7 47.77(5) 1_455 .
Li6 Li13 Li7 123.13(9) 3_666 .
O22 Li13 Li7 135.95(7) . .
O71 Li13 Li7 87.48(8) . 4_575
O71 Li13 Li7 47.06(5) 4_575 4_575
O32 Li13 Li7 137.78(11) . 4_575
O32 Li13 Li7 85.53(5) 4_575 4_575
O63 Li13 Li7 47.77(5) 1_455 4_575
Li6 Li13 Li7 123.13(9) 3_666 4_575
O22 Li13 Li7 135.95(7) . 4_575
Li7 Li13 Li7 62.16(8) . 4_575
O71 Li13 Si7 38.29(4) . .
O71 Li13 Si7 38.29(4) 4_575 .
O32 Li13 Si7 126.77(5) . .
O32 Li13 Si7 126.77(5) 4_575 .
O63 Li13 Si7 99.79(9) 1_455 .
Li6 Li13 Si7 168.86(12) 3_666 .
O22 Li13 Si7 85.57(7) . .
Li7 Li13 Si7 65.87(6) . .
Li7 Li13 Si7 65.87(6) 4_575 .
O71 Li13 Li4 80.95(5) . .
O71 Li13 Li4 127.52(10) 4_575 .
O32 Li13 Li4 44.05(4) . .
O32 Li13 Li4 105.39(9) 4_575 .
O63 Li13 Li4 134.20(6) 1_455 .
Li6 Li13 Li4 67.97(7) 3_666 .
O22 Li13 Li4 43.31(4) . .
Li7 Li13 Li4 109.79(4) . .
Li7 Li13 Li4 168.35(9) 4_575 .
Si7 Li13 Li4 103.59(7) . .
O71 Li13 Li4 127.52(10) . 4_575
O71 Li13 Li4 80.95(5) 4_575 4_575
O32 Li13 Li4 105.39(9) . 4_575
O32 Li13 Li4 44.04(4) 4_575 4_575
O63 Li13 Li4 134.20(6) 1_455 4_575
Li6 Li13 Li4 67.97(7) 3_666 4_575
O22 Li13 Li4 43.31(4) . 4_575
Li7 Li13 Li4 168.36(9) . 4_575
Li7 Li13 Li4 109.79(4) 4_575 4_575
Si7 Li13 Li4 103.59(7) . 4_575
Li4 Li13 Li4 76.74(8) . 4_575
O12 Li14 O22 103.54(7) . .
O12 Li14 O13 81.47(5) . .
O22 Li14 O13 98.92(6) . .
O12 Li14 O72 92.50(6) . .
O22 Li14 O72 103.74(6) . .
O13 Li14 O72 157.33(8) . .
O12 Li14 O71 152.31(8) . .
O22 Li14 O71 103.64(6) . .
O13 Li14 O71 99.38(6) . .
O72 Li14 O71 76.02(5) . .
O12 Li14 Li16 52.47(5) . 2_655
O22 Li14 Li16 137.71(8) . 2_655
O13 Li14 Li16 109.02(7) . 2_655
O72 Li14 Li16 52.08(5) . 2_655
O71 Li14 Li16 102.37(7) . 2_655
O12 Li14 Li4 110.22(7) . .
O22 Li14 Li4 52.26(5) . .
O13 Li14 Li4 50.98(5) . .
O72 Li14 Li4 149.44(7) . .
O71 Li14 Li4 90.66(6) . .
Li16 Li14 Li4 158.27(8) 2_655 .
O12 Li14 Si1 40.14(3) . .
O22 Li14 Si1 104.34(6) . .
O13 Li14 Si1 41.34(3) . .
O72 Li14 Si1 129.37(6) . .
O71 Li14 Si1 134.61(7) . .
Li16 Li14 Si1 79.19(5) 2_655 .
Li4 Li14 Si1 79.28(5) . .
O12 Li14 Li14 102.07(4) . 4_575
O22 Li14 Li14 50.80(4) . 4_575
O13 Li14 Li14 149.67(4) . 4_575
O72 Li14 Li14 52.95(4) . 4_575
O71 Li14 Li14 91.09(4) . 4_575
Li16 Li14 Li14 96.20(4) 2_655 4_575
Li4 Li14 Li14 100.92(5) . 4_575
Si1 Li14 Li14 134.19(3) . 4_575
O12 Li14 Si7 130.31(6) . .
O22 Li14 Si7 98.25(5) . .
O13 Li14 Si7 138.15(7) . .
O72 Li14 Si7 38.61(3) . .
O71 Li14 Si7 39.29(3) . .
Li16 Li14 Si7 81.76(5) 2_655 .
Li4 Li14 Si7 118.42(6) . .
Si1 Li14 Si7 157.13(6) . .
Li14 Li14 Si7 60.42(3) 4_575 .
O12 Li14 Li17 45.73(4) . .
O22 Li14 Li17 62.29(6) . .
O13 Li14 Li17 106.17(6) . .
O72 Li14 Li17 84.14(6) . .
O71 Li14 Li17 152.28(7) . .
Li16 Li14 Li17 79.48(7) 2_655 .
Li4 Li14 Li17 97.06(7) . .
Si1 Li14 Li17 73.10(4) . .
Li14 Li14 Li17 61.34(4) 4_575 .
Si7 Li14 Li17 115.62(6) . .
O12 Li14 Li13 160.42(8) . .
O22 Li14 Li13 57.13(5) . .
O13 Li14 Li13 103.34(6) . .
O72 Li14 Li13 89.66(6) . .
O71 Li14 Li13 46.54(5) . .
Li16 Li14 Li13 138.74(7) 2_655 .
Li4 Li14 Li13 62.11(6) . .
Si1 Li14 Li13 140.92(6) . .
Li14 Li14 Li13 64.21(3) 4_575 .
Si7 Li14 Li13 57.00(5) . .
Li17 Li14 Li13 115.33(7) . .
O73 Li15 O71 112.55(7) . 3_565
O73 Li15 O71 112.55(7) . 2
O71 Li15 O71 113.23(9) 3_565 2
O73 Li15 O72 80.40(7) . .
O71 Li15 O72 116.94(6) 3_565 .
O71 Li15 O72 116.94(6) 2 .
O73 Li15 Li19 130.18(14) . 3_665
O71 Li15 Li19 56.71(5) 3_565 3_665
O71 Li15 Li19 56.71(5) 2 3_665
O72 Li15 Li19 149.41(13) . 3_665
O73 Li15 Si7 40.20(4) . .
O71 Li15 Si7 123.21(5) 3_565 .
O71 Li15 Si7 123.21(5) 2 .
O72 Li15 Si7 40.20(4) . .
Li19 Li15 Si7 170.39(13) 3_665 .
O73 Li15 Li16 107.99(7) . 3_665
O71 Li15 Li16 129.46(9) 3_565 3_665
O71 Li15 Li16 75.58(5) 2 3_665
O72 Li15 Li16 43.33(4) . 3_665
Li19 Li15 Li16 113.84(9) 3_665 3_665
Si7 Li15 Li16 74.09(6) . 3_665
O73 Li15 Li16 107.99(7) . 2_655
O71 Li15 Li16 75.58(5) 3_565 2_655
O71 Li15 Li16 129.46(9) 2 2_655
O72 Li15 Li16 43.33(4) . 2_655
Li19 Li15 Li16 113.84(9) 3_665 2_655
Si7 Li15 Li16 74.09(6) . 2_655
Li16 Li15 Li16 63.97(7) 3_665 2_655
O73 Li15 Li14 73.85(6) . 3_565
O71 Li15 Li14 46.65(5) 3_565 3_565
O71 Li15 Li14 107.65(8) 2 3_565
O72 Li15 Li14 134.35(6) . 3_565
Li19 Li15 Li14 66.54(8) 3_665 3_565
Si7 Li15 Li14 105.99(6) . 3_565
Li16 Li15 Li14 175.54(6) 3_665 3_565
Li16 Li15 Li14 111.66(4) 2_655 3_565
O73 Li15 Li14 73.85(6) . 2
O71 Li15 Li14 107.65(8) 3_565 2
O71 Li15 Li14 46.65(5) 2 2
O72 Li15 Li14 134.35(6) . 2
Li19 Li15 Li14 66.54(8) 3_665 2
Si7 Li15 Li14 105.99(6) . 2
Li16 Li15 Li14 111.66(4) 3_665 2
Li16 Li15 Li14 175.54(6) 2_655 2
Li14 Li15 Li14 72.69(7) 3_565 2
O73 Li15 Si7 90.86(4) . 3_565
O71 Li15 Si7 30.627(15) 3_565 3_565
O71 Li15 Si7 143.79(8) 2 3_565
O72 Li15 Si7 93.16(4) . 3_565
Li19 Li15 Si7 87.11(4) 3_665 3_565
Si7 Li15 Si7 92.63(4) . 3_565
Li16 Li15 Si7 124.49(7) 3_665 3_565
Li16 Li15 Si7 60.56(3) 2_655 3_565
Li14 Li15 Si7 51.11(3) 3_565 3_565
Li14 Li15 Si7 123.76(7) 2 3_565
O73 Li15 Si7 90.86(4) . 3_575
O71 Li15 Si7 143.79(8) 3_565 3_575
O71 Li15 Si7 30.627(15) 2 3_575
O72 Li15 Si7 93.16(4) . 3_575
Li19 Li15 Si7 87.11(4) 3_665 3_575
Si7 Li15 Si7 92.63(4) . 3_575
Li16 Li15 Si7 60.56(3) 3_665 3_575
Li16 Li15 Si7 124.49(7) 2_655 3_575
Li14 Li15 Si7 123.76(7) 3_565 3_575
Li14 Li15 Si7 51.11(3) 2 3_575
Si7 Li15 Si7 173.65(8) 3_565 3_575
O52 Li16 O73 113.67(7) 4_565 1_645
O52 Li16 O12 104.20(6) 4_565 2_645
O73 Li16 O12 111.63(6) 1_645 2_645
O52 Li16 O72 121.38(7) 4_565 3_665
O73 Li16 O72 107.17(6) 1_645 3_665
O12 Li16 O72 97.42(6) 2_645 3_665
O52 Li16 Li14 153.55(8) 4_565 2_645
O73 Li16 Li14 89.87(6) 1_645 2_645
O12 Li16 Li14 53.41(5) 2_645 2_645
O72 Li16 Li14 57.28(5) 3_665 2_645
O52 Li16 Li5 53.51(5) 4_565 4_565
O73 Li16 Li5 129.01(7) 1_645 4_565
O12 Li16 Li5 50.70(4) 2_645 4_565
O72 Li16 Li5 121.30(7) 3_665 4_565
Li14 Li16 Li5 102.68(7) 2_645 4_565
O52 Li16 Li7 43.41(4) 4_565 4_665
O73 Li16 Li7 80.78(5) 1_645 4_665
O12 Li16 Li7 145.51(6) 2_645 4_665
O72 Li16 Li7 109.76(6) 3_665 4_665
Li14 Li16 Li7 161.05(7) 2_645 4_665
Li5 Li16 Li7 95.99(6) 4_565 4_665
O52 Li16 Li15 94.85(6) 4_565 3_665
O73 Li16 Li15 85.96(5) 1_645 3_665
O12 Li16 Li15 145.12(7) 2_645 3_665
O72 Li16 Li15 47.80(5) 3_665 3_665
Li14 Li16 Li15 98.86(6) 2_645 3_665
Li5 Li16 Li15 138.23(7) 4_565 3_665
Li7 Li16 Li15 64.26(5) 4_665 3_665
O52 Li16 Si7 98.81(5) 4_565 1_645
O73 Li16 Si7 28.40(3) 1_645 1_645
O12 Li16 Si7 140.02(6) 2_645 1_645
O72 Li16 Si7 97.85(5) 3_665 1_645
Li14 Li16 Si7 107.59(6) 2_645 1_645
Li5 Li16 Si7 139.46(6) 4_565 1_645
Li7 Li16 Si7 57.88(4) 4_665 1_645
Li15 Li16 Si7 62.03(3) 3_665 1_645
O52 Li16 Li16 95.52(4) 4_565 4
O73 Li16 Li16 38.36(4) 1_645 4
O12 Li16 Li16 85.38(4) 2_645 4
O72 Li16 Li16 140.52(4) 3_665 4
Li14 Li16 Li16 96.20(4) 2_645 4
Li5 Li16 Li16 90.81(4) 4_565 4
Li7 Li16 Li16 86.67(4) 4_665 4
Li15 Li16 Li16 121.99(3) 3_665 4
Si7 Li16 Li16 60.00(2) 1_645 4
O52 Li16 Li16 84.48(4) 4_565 4_565
O73 Li16 Li16 141.64(4) 1_645 4_565
O12 Li16 Li16 94.62(4) 2_645 4_565
O72 Li16 Li16 39.48(4) 3_665 4_565
Li14 Li16 Li16 83.80(4) 2_645 4_565
Li5 Li16 Li16 89.19(4) 4_565 4_565
Li7 Li16 Li16 93.33(4) 4_665 4_565
Li15 Li16 Li16 58.01(3) 3_665 4_565
Si7 Li16 Li16 120.00(2) 1_645 4_565
Li16 Li16 Li16 180.0 4 4_565
O52 Li16 Si1 115.11(5) 4_565 3_655
O73 Li16 Si1 85.19(5) 1_645 3_655
O12 Li16 Si1 26.52(2) 2_645 3_655
O72 Li16 Si1 108.33(5) 3_665 3_655
Li14 Li16 Si1 52.36(4) 2_645 3_655
Li5 Li16 Si1 66.32(4) 4_565 3_655
Li7 Li16 Si1 141.77(5) 4_665 3_655
Li15 Li16 Si1 149.82(6) 3_665 3_655
Si7 Li16 Si1 113.57(4) 1_645 3_655
Li16 Li16 Si1 61.34(2) 4 3_655
Li16 Li16 Si1 118.66(2) 4_565 3_655
O12 Li17 O12 124.60(11) . 4_575
O12 Li17 O21 116.48(6) . .
O12 Li17 O21 116.48(6) 4_575 .
O12 Li17 O22 90.47(8) . .
O12 Li17 O22 90.47(8) 4_575 .
O21 Li17 O22 72.55(7) . .
O12 Li17 Li14 100.41(9) . 4_575
O12 Li17 Li14 48.04(5) 4_575 4_575
O21 Li17 Li14 107.73(9) . 4_575
O22 Li17 Li14 46.07(5) . 4_575
O12 Li17 Li14 48.04(5) . .
O12 Li17 Li14 100.40(9) 4_575 .
O21 Li17 Li14 107.73(9) . .
O22 Li17 Li14 46.07(5) . .
Li14 Li17 Li14 57.31(7) 4_575 .
O12 Li17 Li5 45.72(5) . 3_665
O12 Li17 Li5 105.69(9) 4_575 3_665
O21 Li17 Li5 129.73(8) . 3_665
O22 Li17 Li5 135.03(7) . 3_665
Li14 Li17 Li5 120.84(9) 4_575 3_665
Li14 Li17 Li5 89.31(6) . 3_665
O12 Li17 Li5 105.69(9) . 2_655
O12 Li17 Li5 45.72(5) 4_575 2_655
O21 Li17 Li5 129.73(8) . 2_655
O22 Li17 Li5 135.03(7) . 2_655
Li14 Li17 Li5 89.31(6) 4_575 2_655
Li14 Li17 Li5 120.84(9) . 2_655
Li5 Li17 Li5 66.32(7) 3_665 2_655
O12 Li17 Si2 106.54(7) . .
O12 Li17 Si2 106.53(7) 4_575 .
O21 Li17 Si2 35.81(4) . .
O22 Li17 Si2 36.74(4) . .
Li14 Li17 Si2 76.43(7) 4_575 .
Li14 Li17 Si2 76.43(7) . .
Li5 Li17 Si2 146.58(4) 3_665 .
Li5 Li17 Si2 146.58(4) 2_655 .
O12 Li17 Li5 83.23(4) . .
O12 Li17 Li5 150.17(9) 4_575 .
O21 Li17 Li5 44.21(4) . .
O22 Li17 Li5 100.72(7) . .
Li14 Li17 Li5 146.20(10) 4_575 .
Li14 Li17 Li5 107.29(5) . .
Li5 Li17 Li5 85.79(6) 3_665 .
Li5 Li17 Li5 122.37(9) 2_655 .
Si2 Li17 Li5 70.40(5) . .
O12 Li17 Li5 150.17(9) . 4_575
O12 Li17 Li5 83.23(4) 4_575 4_575
O21 Li17 Li5 44.21(4) . 4_575
O22 Li17 Li5 100.71(7) . 4_575
Li14 Li17 Li5 107.29(5) 4_575 4_575
Li14 Li17 Li5 146.20(10) . 4_575
Li5 Li17 Li5 122.37(9) 3_665 4_575
Li5 Li17 Li5 85.79(6) 2_655 4_575
Si2 Li17 Li5 70.40(5) . 4_575
Li5 Li17 Li5 67.62(7) . 4_575
O12 Li17 Si1 147.69(10) . 1_565
O12 Li17 Si1 26.64(2) 4_575 1_565
O21 Li17 Si1 89.93(4) . 1_565
O22 Li17 Si1 79.61(4) . 1_565
Li14 Li17 Si1 51.25(3) 4_575 1_565
Li14 Li17 Si1 108.42(7) . 1_565
Li5 Li17 Si1 129.78(7) 3_665 1_565
Li5 Li17 Si1 64.25(3) 2_655 1_565
Si2 Li17 Si1 83.61(4) . 1_565
Li5 Li17 Si1 128.68(7) . 1_565
Li5 Li17 Si1 62.10(3) 4_575 1_565
O62 Li18 O62 75.17(8) 3_666 2_646
O62 Li18 O62 165.59(9) 3_666 4_465
O62 Li18 O62 90.53(2) 2_646 4_465
O62 Li18 O62 90.53(2) 3_666 1_455
O62 Li18 O62 165.59(9) 2_646 1_455
O62 Li18 O62 103.70(10) 4_465 1_455
O62 Li18 O33 92.91(10) 3_666 .
O62 Li18 O33 92.91(10) 2_646 .
O62 Li18 O33 89.57(9) 4_465 .
O62 Li18 O33 89.57(9) 1_455 .
O62 Li18 Li12 142.21(4) 3_666 1_455
O62 Li18 Li12 142.21(4) 2_646 1_455
O62 Li18 Li12 51.86(5) 4_465 1_455
O62 Li18 Li12 51.86(5) 1_455 1_455
O33 Li18 Li12 90.52(11) . 1_455
O62 Li18 O43 93.45(9) 3_666 1_455
O62 Li18 O43 93.45(9) 2_646 1_455
O62 Li18 O43 85.48(8) 4_465 1_455
O62 Li18 O43 85.48(8) 1_455 1_455
O33 Li18 O43 171.97(12) . 1_455
Li12 Li18 O43 81.45(9) 1_455 1_455
O62 Li18 Li9 46.69(5) 3_666 2_656
O62 Li18 Li9 86.22(9) 2_646 2_656
O62 Li18 Li9 135.67(13) 4_465 2_656
O62 Li18 Li9 85.19(6) 1_455 2_656
O33 Li18 Li9 46.61(6) . 2_656
Li12 Li18 Li9 121.72(11) 1_455 2_656
O43 Li18 Li9 138.83(8) 1_455 2_656
O62 Li18 Li9 86.22(9) 3_666 3_656
O62 Li18 Li9 46.69(5) 2_646 3_656
O62 Li18 Li9 85.19(6) 4_465 3_656
O62 Li18 Li9 135.67(13) 1_455 3_656
O33 Li18 Li9 46.61(6) . 3_656
Li12 Li18 Li9 121.72(11) 1_455 3_656
O43 Li18 Li9 138.83(8) 1_455 3_656
Li9 Li18 Li9 61.08(9) 2_656 3_656
O62 Li18 Si6 37.78(4) 3_666 3_666
O62 Li18 Si6 37.78(4) 2_646 3_666
O62 Li18 Si6 127.81(5) 4_465 3_666
O62 Li18 Si6 127.81(5) 1_455 3_666
O33 Li18 Si6 97.77(9) . 3_666
Li12 Li18 Si6 171.71(14) 1_455 3_666
O43 Li18 Si6 90.26(9) 1_455 3_666
Li9 Li18 Si6 65.05(6) 2_656 3_666
Li9 Li18 Si6 65.05(6) 3_656 3_666
O62 Li18 Li9 129.44(12) 3_666 1_455
O62 Li18 Li9 82.63(6) 2_646 1_455
O62 Li18 Li9 44.58(5) 4_465 1_455
O62 Li18 Li9 105.78(10) 1_455 1_455
O33 Li18 Li9 133.58(7) . 1_455
Li12 Li18 Li9 68.22(7) 1_455 1_455
O43 Li18 Li9 42.81(5) 1_455 1_455
Li9 Li18 Li9 168.84(9) 2_656 1_455
Li9 Li18 Li9 110.18(4) 3_656 1_455
Si6 Li18 Li9 105.56(8) 3_666 1_455
O62 Li18 Li9 82.63(6) 3_666 4_465
O62 Li18 Li9 129.44(12) 2_646 4_465
O62 Li18 Li9 105.78(10) 4_465 4_465
O62 Li18 Li9 44.58(5) 1_455 4_465
O33 Li18 Li9 133.58(7) . 4_465
Li12 Li18 Li9 68.22(7) 1_455 4_465
O43 Li18 Li9 42.81(5) 1_455 4_465
Li9 Li18 Li9 110.18(4) 2_656 4_465
Li9 Li18 Li9 168.84(9) 3_656 4_465
Si6 Li18 Li9 105.56(8) 3_666 4_465
Li9 Li18 Li9 77.49(9) 1_455 4_465
O71 Li19 O71 106.18(11) 4_665 1_655
O71 Li19 O32 164.41(10) 4_665 1_655
O71 Li19 O32 89.22(2) 1_655 1_655
O71 Li19 O32 89.22(2) 4_665 4_665
O71 Li19 O32 164.41(10) 1_655 4_665
O32 Li19 O32 75.30(8) 1_655 4_665
O71 Li19 Li15 53.17(5) 4_665 3_665
O71 Li19 Li15 53.17(5) 1_655 3_665
O32 Li19 Li15 141.85(5) 1_655 3_665
O32 Li19 Li15 141.85(5) 4_665 3_665
O71 Li19 O53 87.51(9) 4_665 .
O71 Li19 O53 87.51(9) 1_655 .
O32 Li19 O53 95.78(11) 1_655 .
O32 Li19 O53 95.78(11) 4_665 .
Li15 Li19 O53 89.35(11) 3_665 .
O71 Li19 O13 88.35(10) 4_665 1_655
O71 Li19 O13 88.35(10) 1_655 1_655
O32 Li19 O13 89.68(10) 1_655 1_655
O32 Li19 O13 89.68(10) 4_665 1_655
Li15 Li19 O13 83.74(11) 3_665 1_655
O53 Li19 O13 173.09(12) . 1_655
O71 Li19 Li7 45.65(5) 4_665 4_665
O71 Li19 Li7 108.85(11) 1_655 4_665
O32 Li19 Li7 131.95(14) 1_655 4_665
O32 Li19 Li7 83.55(7) 4_665 4_665
Li15 Li19 Li7 74.36(8) 3_665 4_665
O53 Li19 Li7 43.67(6) . 4_665
O13 Li19 Li7 133.36(8) 1_655 4_665
O71 Li19 Li7 108.85(11) 4_665 1_655
O71 Li19 Li7 45.65(5) 1_655 1_655
O32 Li19 Li7 83.55(7) 1_655 1_655
O32 Li19 Li7 131.95(14) 4_665 1_655
Li15 Li19 Li7 74.36(8) 3_665 1_655
O53 Li19 Li7 43.67(6) . 1_655
O13 Li19 Li7 133.36(8) 1_655 1_655
Li7 Li19 Li7 79.46(10) 4_665 1_655
O71 Li19 Li4 131.85(14) 4_665 1_655
O71 Li19 Li4 83.58(7) 1_655 1_655
O32 Li19 Li4 45.95(6) 1_655 1_655
O32 Li19 Li4 84.25(9) 4_665 1_655
Li15 Li19 Li4 114.59(12) 3_665 1_655
O53 Li19 Li4 140.58(9) . 1_655
O13 Li19 Li4 44.12(6) 1_655 1_655
Li7 Li19 Li4 167.57(9) 4_665 1_655
Li7 Li19 Li4 110.72(4) 1_655 1_655
O71 Li19 Li4 83.58(7) 4_665 4_665
O71 Li19 Li4 131.85(14) 1_655 4_665
O32 Li19 Li4 84.25(9) 1_655 4_665
O32 Li19 Li4 45.95(6) 4_665 4_665
Li15 Li19 Li4 114.59(12) 3_665 4_665
O53 Li19 Li4 140.58(9) . 4_665
O13 Li19 Li4 44.12(6) 1_655 4_665
Li7 Li19 Li4 110.72(4) 4_665 4_665
Li7 Li19 Li4 167.57(9) 1_655 4_665
Li4 Li19 Li4 58.30(9) 1_655 4_665
O71 Li19 Si3 126.90(5) 4_665 1_655
O71 Li19 Si3 126.90(5) 1_655 1_655
O32 Li19 Si3 37.89(4) 1_655 1_655
O32 Li19 Si3 37.89(4) 4_665 1_655
Li15 Li19 Si3 177.95(16) 3_665 1_655
O53 Li19 Si3 92.69(10) . 1_655
O13 Li19 Si3 94.21(10) 1_655 1_655
Li7 Li19 Si3 107.16(9) 4_665 1_655
Li7 Li19 Si3 107.16(9) 1_655 1_655
Li4 Li19 Si3 63.69(6) 1_655 1_655
Li4 Li19 Si3 63.69(6) 4_665 1_655
O11 Si1 O12 111.20(2) . 4_565
O11 Si1 O12 111.20(2) . .
O12 Si1 O12 111.16(3) 4_565 .
O11 Si1 O13 111.81(4) . .
O12 Si1 O13 105.60(2) 4_565 .
O12 Si1 O13 105.60(2) . .
O11 Si1 Li14 126.43(4) . 4_565
O12 Si1 Li14 52.03(3) 4_565 4_565
O12 Si1 Li14 122.34(4) . 4_565
O13 Si1 Li14 53.58(3) . 4_565
O11 Si1 Li14 126.43(4) . .
O12 Si1 Li14 122.34(4) 4_565 .
O12 Si1 Li14 52.03(3) . .
O13 Si1 Li14 53.58(3) . .
Li14 Si1 Li14 88.39(7) 4_565 .
O11 Si1 Li11 39.64(4) . .
O12 Si1 Li11 123.753(17) 4_565 .
O12 Si1 Li11 123.753(18) . .
O13 Si1 Li11 72.16(4) . .
Li14 Si1 Li11 101.59(4) 4_565 .
Li14 Si1 Li11 101.59(4) . .
O11 Si1 Li5 31.96(2) . .
O12 Si1 Li5 129.40(3) 4_565 .
O12 Si1 Li5 79.47(3) . .
O13 Si1 Li5 119.21(3) . .
Li14 Si1 Li5 157.52(4) 4_565 .
Li14 Si1 Li5 103.48(4) . .
Li11 Si1 Li5 57.68(4) . .
O11 Si1 Li5 31.96(2) . 4_565
O12 Si1 Li5 79.47(3) 4_565 4_565
O12 Si1 Li5 129.40(3) . 4_565
O13 Si1 Li5 119.21(3) . 4_565
Li14 Si1 Li5 103.48(4) 4_565 4_565
Li14 Si1 Li5 157.52(4) . 4_565
Li11 Si1 Li5 57.68(4) . 4_565
Li5 Si1 Li5 59.41(5) . 4_565
O11 Si1 Li17 84.80(4) . 1_545
O12 Si1 Li17 31.88(4) 4_565 1_545
O12 Si1 Li17 140.45(4) . 1_545
O13 Si1 Li17 100.80(4) . 1_545
Li14 Si1 Li17 55.65(5) 4_565 1_545
Li14 Si1 Li17 143.60(5) . 1_545
Li11 Si1 Li17 92.05(4) . 1_545
Li5 Si1 Li17 112.26(5) . 1_545
Li5 Si1 Li17 53.53(5) 4_565 1_545
O11 Si1 Li17 84.80(4) . .
O12 Si1 Li17 140.45(4) 4_565 .
O12 Si1 Li17 31.88(4) . .
O13 Si1 Li17 100.80(4) . .
Li14 Si1 Li17 143.60(5) 4_565 .
Li14 Si1 Li17 55.65(5) . .
Li11 Si1 Li17 92.05(4) . .
Li5 Si1 Li17 53.53(5) . .
Li5 Si1 Li17 112.26(5) 4_565 .
Li17 Si1 Li17 158.25(9) 1_545 .
O11 Si1 Li5 99.83(3) . 2_645
O12 Si1 Li5 33.01(3) 4_565 2_645
O12 Si1 Li5 88.48(3) . 2_645
O13 Si1 Li5 136.81(3) . 2_645
Li14 Si1 Li5 84.18(4) 4_565 2_645
Li14 Si1 Li5 125.79(4) . 2_645
Li11 Si1 Li5 132.54(4) . 2_645
Li5 Si1 Li5 103.29(2) . 2_645
Li5 Si1 Li5 75.05(4) 4_565 2_645
Li17 Si1 Li5 52.48(5) 1_545 2_645
Li17 Si1 Li5 110.95(5) . 2_645
Si1 O11 Li5 120.99(4) . .
Si1 O11 Li5 120.99(4) . 4_565
Li5 O11 Li5 106.74(8) . 4_565
Si1 O11 Li11 108.65(6) . .
Li5 O11 Li11 96.94(5) . .
Li5 O11 Li11 96.94(5) 4_565 .
Si1 O12 Li17 121.48(6) . .
Si1 O12 Li16 120.83(4) . 2_655
Li17 O12 Li16 113.08(7) . 2_655
Si1 O12 Li5 120.20(4) . 3_665
Li17 O12 Li5 90.07(8) . 3_665
Li16 O12 Li5 78.68(5) 2_655 3_665
Si1 O12 Li14 87.83(4) . .
Li17 O12 Li14 86.23(8) . .
Li16 O12 Li14 74.11(6) 2_655 .
Li5 O12 Li14 148.48(6) 3_665 .
Si1 O13 Li4 120.80(4) . .
Si1 O13 Li4 120.80(4) . 4_565
Li4 O13 Li4 84.88(8) . 4_565
Si1 O13 Li14 85.08(4) . 4_565
Li4 O13 Li14 152.98(6) . 4_565
Li4 O13 Li14 74.10(5) 4_565 4_565
Si1 O13 Li14 85.08(4) . .
Li4 O13 Li14 74.10(5) . .
Li4 O13 Li14 152.98(6) 4_565 .
Li14 O13 Li14 119.33(9) 4_565 .
Si1 O13 Li19 157.05(7) . 1_455
Li4 O13 Li19 74.67(6) . 1_455
Li4 O13 Li19 74.67(6) 4_565 1_455
Li14 O13 Li19 83.39(5) 4_565 1_455
Li14 O13 Li19 83.39(5) . 1_455
O21 Si2 O23 112.09(2) . .
O21 Si2 O23 112.09(2) . 4_575
O23 Si2 O23 110.93(3) . 4_575
O21 Si2 O22 110.71(3) . .
O23 Si2 O22 105.30(2) . .
O23 Si2 O22 105.30(2) 4_575 .
O21 Si2 Li4 124.26(3) . 4_575
O23 Si2 Li4 123.55(3) . 4_575
O23 Si2 Li4 51.96(4) 4_575 4_575
O22 Si2 Li4 53.44(3) . 4_575
O21 Si2 Li4 124.26(3) . .
O23 Si2 Li4 51.96(4) . .
O23 Si2 Li4 123.55(3) 4_575 .
O22 Si2 Li4 53.44(3) . .
Li4 Si2 Li4 90.38(6) 4_575 .
O21 Si2 Li17 47.50(5) . .
O23 Si2 Li17 124.531(17) . .
O23 Si2 Li17 124.533(17) 4_575 .
O22 Si2 Li17 63.21(5) . .
Li4 Si2 Li17 93.88(5) 4_575 .
Li4 Si2 Li17 93.88(5) . .
O21 Si2 Li3 42.03(4) . .
O23 Si2 Li3 89.73(3) . .
O23 Si2 Li3 89.73(3) 4_575 .
O22 Si2 Li3 152.74(4) . .
Li4 Si2 Li3 134.59(3) 4_575 .
Li4 Si2 Li3 134.59(3) . .
Li17 Si2 Li3 89.53(6) . .
O21 Si2 Li10 92.55(3) . 4_575
O23 Si2 Li10 37.86(3) . 4_575
O23 Si2 Li10 90.99(3) 4_575 4_575
O22 Si2 Li10 143.01(3) . 4_575
Li4 Si2 Li10 133.76(4) 4_575 4_575
Li4 Si2 Li10 89.82(4) . 4_575
Li17 Si2 Li10 132.22(4) . 4_575
Li3 Si2 Li10 56.63(4) . 4_575
O21 Si2 Li10 92.55(3) . .
O23 Si2 Li10 90.99(3) . .
O23 Si2 Li10 37.86(3) 4_575 .
O22 Si2 Li10 143.01(3) . .
Li4 Si2 Li10 89.82(4) 4_575 .
Li4 Si2 Li10 133.76(4) . .
Li17 Si2 Li10 132.22(4) . .
Li3 Si2 Li10 56.63(4) . .
Li10 Si2 Li10 58.64(5) 4_575 .
O21 Si2 Li11 82.40(3) . .
O23 Si2 Li11 32.98(4) . .
O23 Si2 Li11 139.01(4) 4_575 .
O22 Si2 Li11 104.42(3) . .
Li4 Si2 Li11 148.48(5) 4_575 .
Li4 Si2 Li11 58.66(4) . .
Li17 Si2 Li11 94.02(4) . .
Li3 Si2 Li11 75.93(3) . .
Li10 Si2 Li11 48.99(4) 4_575 .
Li10 Si2 Li11 106.93(4) . .
O21 Si2 Li11 82.40(3) . 1_565
O23 Si2 Li11 139.01(4) . 1_565
O23 Si2 Li11 32.98(4) 4_575 1_565
O22 Si2 Li11 104.42(3) . 1_565
Li4 Si2 Li11 58.66(4) 4_575 1_565
Li4 Si2 Li11 148.48(5) . 1_565
Li17 Si2 Li11 94.02(4) . 1_565
Li3 Si2 Li11 75.93(3) . 1_565
Li10 Si2 Li11 106.93(4) 4_575 1_565
Li10 Si2 Li11 48.99(4) . 1_565
Li11 Si2 Li11 150.63(7) . 1_565
Si2 O21 Li5 127.02(4) . 4_575
Si2 O21 Li5 127.02(4) . .
Li5 O21 Li5 105.79(8) 4_575 .
Si2 O21 Li17 96.69(7) . .
Li5 O21 Li17 88.16(6) 4_575 .
Li5 O21 Li17 88.16(6) . .
Si2 O21 Li3 106.34(6) . .
Li5 O21 Li3 78.10(5) 4_575 .
Li5 O21 Li3 78.10(5) . .
Li17 O21 Li3 156.97(9) . .
Si2 O22 Li4 83.80(4) . .
Si2 O22 Li4 83.80(4) . 4_575
Li4 O22 Li4 122.83(8) . 4_575
Si2 O22 Li14 130.02(4) . .
Li4 O22 Li14 73.50(5) . .
Li4 O22 Li14 145.69(6) 4_575 .
Si2 O22 Li14 130.02(4) . 4_575
Li4 O22 Li14 145.69(6) . 4_575
Li4 O22 Li14 73.50(5) 4_575 4_575
Li14 O22 Li14 78.39(8) . 4_575
Si2 O22 Li17 80.05(5) . .
Li4 O22 Li17 116.13(4) . .
Li4 O22 Li17 116.13(4) 4_575 .
Li14 O22 Li17 71.64(6) . .
Li14 O22 Li17 71.64(6) 4_575 .
Si2 O22 Li13 136.66(6) . .
Li4 O22 Li13 76.03(5) . .
Li4 O22 Li13 76.03(5) 4_575 .
Li14 O22 Li13 80.16(6) . .
Li14 O22 Li13 80.16(6) 4_575 .
Li17 O22 Li13 143.29(7) . .
Si2 O23 Li4 86.38(4) . .
Si2 O23 Li2 127.59(4) . .
Li4 O23 Li2 90.93(6) . .
Si2 O23 Li11 120.50(5) . .
Li4 O23 Li11 91.47(7) . .
Li2 O23 Li11 111.88(6) . .
Si2 O23 Li10 112.04(4) . 4_575
Li4 O23 Li10 161.57(6) . 4_575
Li2 O23 Li10 77.51(6) . 4_575
Li11 O23 Li10 79.88(7) . 4_575
O31 Si3 O33 114.47(4) . .
O31 Si3 O32 111.13(2) . 4_565
O33 Si3 O32 106.57(2) . 4_565
O31 Si3 O32 111.13(2) . .
O33 Si3 O32 106.57(2) . .
O32 Si3 O32 106.52(3) 4_565 .
O31 Si3 Li1 136.51(7) . .
O33 Si3 Li1 53.47(4) . .
O32 Si3 Li1 112.31(7) 4_565 .
O32 Si3 Li1 53.59(4) . .
O31 Si3 Li1 136.51(7) . 4_565
O33 Si3 Li1 53.47(4) . 4_565
O32 Si3 Li1 53.59(4) 4_565 4_565
O32 Si3 Li1 112.31(7) . 4_565
Li1 Si3 Li1 74.78(12) . 4_565
O31 Si3 Li19 135.09(8) . 1_455
O33 Si3 Li19 110.44(8) . 1_455
O32 Si3 Li19 53.678(19) 4_565 1_455
O32 Si3 Li19 53.678(19) . 1_455
Li1 Si3 Li19 73.43(8) . 1_455
Li1 Si3 Li19 73.43(8) 4_565 1_455
O31 Si3 Li4 82.59(3) . 4_565
O33 Si3 Li4 148.47(3) . 4_565
O32 Si3 Li4 42.08(3) 4_565 4_565
O32 Si3 Li4 89.85(3) . 4_565
Li1 Si3 Li4 131.15(6) . 4_565
Li1 Si3 Li4 95.61(5) 4_565 4_565
Li19 Si3 Li4 58.11(7) 1_455 4_565
O31 Si3 Li4 82.59(3) . .
O33 Si3 Li4 148.47(3) . .
O32 Si3 Li4 89.85(3) 4_565 .
O32 Si3 Li4 42.08(3) . .
Li1 Si3 Li4 95.61(5) . .
Li1 Si3 Li4 131.15(6) 4_565 .
Li19 Si3 Li4 58.11(7) 1_455 .
Li4 Si3 Li4 54.96(5) 4_565 .
O31 Si3 Li8 35.83(4) . .
O33 Si3 Li8 78.63(4) . .
O32 Si3 Li8 124.870(19) 4_565 .
O32 Si3 Li8 124.870(19) . .
Li1 Si3 Li8 113.49(7) . .
Li1 Si3 Li8 113.49(7) 4_565 .
Li19 Si3 Li8 170.92(8) 1_455 .
Li4 Si3 Li8 114.16(4) 4_565 .
Li4 Si3 Li8 114.16(4) . .
O31 Si3 Li2 33.51(3) . .
O33 Si3 Li2 124.66(3) . .
O32 Si3 Li2 125.44(3) 4_565 .
O32 Si3 Li2 77.71(3) . .
Li1 Si3 Li2 112.59(7) . .
Li1 Si3 Li2 169.97(8) 4_565 .
Li19 Si3 Li2 114.66(7) 1_455 .
Li4 Si3 Li2 84.56(4) 4_565 .
Li4 Si3 Li2 56.55(4) . .
Li8 Si3 Li2 57.84(4) . .
O31 Si3 Li2 33.51(3) . 4_565
O33 Si3 Li2 124.66(3) . 4_565
O32 Si3 Li2 77.71(3) 4_565 4_565
O32 Si3 Li2 125.43(3) . 4_565
Li1 Si3 Li2 169.97(8) . 4_565
Li1 Si3 Li2 112.59(7) 4_565 4_565
Li19 Si3 Li2 114.66(7) 1_455 4_565
Li4 Si3 Li2 56.55(4) 4_565 4_565
Li4 Si3 Li2 84.56(4) . 4_565
Li8 Si3 Li2 57.84(4) . 4_565
Li2 Si3 Li2 59.28(5) . 4_565
Si3 O31 Li2 118.81(5) . 4_565
Si3 O31 Li2 118.81(5) . .
Li2 O31 Li2 103.42(8) 4_565 .
Si3 O31 Li8 114.82(7) . .
Li2 O31 Li8 98.69(6) 4_565 .
Li2 O31 Li8 98.70(6) . .
Si3 O32 Li4 103.40(5) . .
Si3 O32 Li6 112.03(5) . 3_666
Li4 O32 Li6 94.48(7) . 3_666
Si3 O32 Li1 85.93(5) . .
Li4 O32 Li1 170.03(7) . .
Li6 O32 Li1 85.09(10) 3_666 .
Si3 O32 Li19 88.43(5) . 1_455
Li4 O32 Li19 81.18(10) . 1_455
Li6 O32 Li19 159.51(7) 3_666 1_455
Li1 O32 Li19 95.75(13) . 1_455
Si3 O32 Li13 170.85(7) . .
Li4 O32 Li13 85.29(7) . .
Li6 O32 Li13 69.51(6) 3_666 .
Li1 O32 Li13 85.23(8) . .
Li19 O32 Li13 90.12(6) 1_455 .
Si3 O33 Li9 113.66(5) . 2_656
Si3 O33 Li9 113.66(4) . 3_656
Li9 O33 Li9 85.70(9) 2_656 3_656
Si3 O33 Li1 86.14(5) . 4_565
Li9 O33 Li1 160.17(7) 2_656 4_565
Li9 O33 Li1 85.13(9) 3_656 4_565
Si3 O33 Li1 86.14(5) . .
Li9 O33 Li1 85.13(9) 2_656 .
Li9 O33 Li1 160.17(7) 3_656 .
Li1 O33 Li1 97.87(18) 4_565 .
Si3 O33 Li18 165.32(7) . .
Li9 O33 Li18 76.54(6) 2_656 .
Li9 O33 Li18 76.54(6) 3_656 .
Li1 O33 Li18 84.23(6) 4_565 .
Li1 O33 Li18 84.23(6) . .
O42 Si4 O42 113.41(3) 4_565 .
O42 Si4 O41 112.33(2) 4_565 .
O42 Si4 O41 112.33(2) . .
O42 Si4 O43 105.79(2) 4_565 .
O42 Si4 O43 105.79(2) . .
O41 Si4 O43 106.48(3) . .
O42 Si4 Li9 54.09(4) 4_565 .
O42 Si4 Li9 125.85(4) . .
O41 Si4 Li9 121.01(3) . .
O43 Si4 Li9 51.76(4) . .
O42 Si4 Li9 125.85(4) 4_565 4_565
O42 Si4 Li9 54.10(4) . 4_565
O41 Si4 Li9 121.01(3) . 4_565
O43 Si4 Li9 51.76(4) . 4_565
Li9 Si4 Li9 89.03(6) . 4_565
O42 Si4 Li6 123.077(17) 4_565 .
O42 Si4 Li6 123.078(17) . .
O41 Si4 Li6 52.35(5) . .
O43 Si4 Li6 54.13(6) . .
Li9 Si4 Li6 85.66(5) . .
Li9 Si4 Li6 85.66(5) 4_565 .
O42 Si4 Li8 92.11(3) 4_565 .
O42 Si4 Li8 92.11(3) . .
O41 Si4 Li8 39.96(4) . .
O43 Si4 Li8 146.44(4) . .
Li9 Si4 Li8 135.36(3) . .
Li9 Si4 Li8 135.36(3) 4_565 .
Li6 Si4 Li8 92.30(6) . .
O42 Si4 Li2 39.12(3) 4_565 4_565
O42 Si4 Li2 93.53(3) . 4_565
O41 Si4 Li2 92.20(3) . 4_565
O43 Si4 Li2 144.91(3) . 4_565
Li9 Si4 Li2 93.17(4) . 4_565
Li9 Si4 Li2 139.27(4) 4_565 4_565
Li6 Si4 Li2 135.07(4) . 4_565
Li8 Si4 Li2 58.27(4) . 4_565
O42 Si4 Li2 93.53(3) 4_565 .
O42 Si4 Li2 39.12(3) . .
O41 Si4 Li2 92.20(3) . .
O43 Si4 Li2 144.91(3) . .
Li9 Si4 Li2 139.27(4) . .
Li9 Si4 Li2 93.17(4) 4_565 .
Li6 Si4 Li2 135.07(4) . .
Li8 Si4 Li2 58.27(4) . .
Li2 Si4 Li2 60.12(5) 4_565 .
O42 Si4 Li8 32.15(4) 4_565 3_656
O42 Si4 Li8 140.51(4) . 3_656
O41 Si4 Li8 82.71(3) . 3_656
O43 Si4 Li8 104.08(3) . 3_656
Li9 Si4 Li8 59.55(5) . 3_656
Li9 Si4 Li8 148.28(5) 4_565 3_656
Li6 Si4 Li8 95.38(4) . 3_656
Li8 Si4 Li8 76.35(3) . 3_656
Li2 Si4 Li8 48.16(4) 4_565 3_656
Li2 Si4 Li8 107.63(4) . 3_656
O42 Si4 Li8 140.51(4) 4_565 3_666
O42 Si4 Li8 32.15(4) . 3_666
O41 Si4 Li8 82.71(3) . 3_666
O43 Si4 Li8 104.08(3) . 3_666
Li9 Si4 Li8 148.28(5) . 3_666
Li9 Si4 Li8 59.55(5) 4_565 3_666
Li6 Si4 Li8 95.38(4) . 3_666
Li8 Si4 Li8 76.35(3) . 3_666
Li2 Si4 Li8 107.63(4) 4_565 3_666
Li2 Si4 Li8 48.16(4) . 3_666
Li8 Si4 Li8 150.97(7) 3_656 3_666
Si4 O41 Li2 126.60(4) . 3_666
Si4 O41 Li2 126.60(4) . 2_646
Li2 O41 Li2 106.79(8) 3_666 2_646
Si4 O41 Li6 86.23(7) . .
Li2 O41 Li6 92.44(6) 3_666 .
Li2 O41 Li6 92.44(6) 2_646 .
Si4 O41 Li8 108.68(6) . .
Li2 O41 Li8 78.80(5) 3_666 .
Li2 O41 Li8 78.80(5) 2_646 .
Li6 O41 Li8 165.10(8) . .
Si4 O42 Li10 127.18(5) . 4_575
Si4 O42 Li8 121.82(5) . 3_666
Li10 O42 Li8 110.97(6) 4_575 3_666
Si4 O42 Li9 84.56(4) . 4_565
Li10 O42 Li9 95.91(6) 4_575 4_565
Li8 O42 Li9 91.71(7) 3_666 4_565
Si4 O42 Li2 110.02(4) . .
Li10 O42 Li2 77.91(6) 4_575 .
Li8 O42 Li2 78.19(7) 3_666 .
Li9 O42 Li2 165.12(6) 4_565 .
Si4 O43 Li9 85.31(5) . 4_565
Si4 O43 Li9 85.31(5) . .
Li9 O43 Li9 125.65(8) 4_565 .
Si4 O43 Li6 83.20(6) . .
Li9 O43 Li6 115.88(4) 4_565 .
Li9 O43 Li6 115.88(4) . .
Si4 O43 Li18 135.24(6) . 1_655
Li9 O43 Li18 75.03(5) 4_565 1_655
Li9 O43 Li18 75.03(5) . 1_655
Li6 O43 Li18 141.56(9) . 1_655
Si4 O43 Li1 135.75(4) . 3_666
Li9 O43 Li1 72.70(5) 4_565 3_666
Li9 O43 Li1 138.65(6) . 3_666
Li6 O43 Li1 73.34(6) . 3_666
Li18 O43 Li1 75.81(6) 1_655 3_666
Si4 O43 Li1 135.75(4) . 2_646
Li9 O43 Li1 138.65(6) 4_565 2_646
Li9 O43 Li1 72.70(5) . 2_646
Li6 O43 Li1 73.34(6) . 2_646
Li18 O43 Li1 75.81(6) 1_655 2_646
Li1 O43 Li1 72.18(7) 3_666 2_646
O51 Si5 O52 112.17(2) . .
O51 Si5 O52 112.17(2) . 4_565
O52 Si5 O52 113.45(3) . 4_565
O51 Si5 O53 106.45(3) . .
O52 Si5 O53 105.97(2) . .
O52 Si5 O53 105.97(2) 4_565 .
O51 Si5 Li7 120.62(3) . 1_655
O52 Si5 Li7 54.57(4) . 1_655
O52 Si5 Li7 126.35(4) 4_565 1_655
O53 Si5 Li7 51.48(4) . 1_655
O51 Si5 Li7 120.62(3) . 4_665
O52 Si5 Li7 126.35(4) . 4_665
O52 Si5 Li7 54.57(4) 4_565 4_665
O53 Si5 Li7 51.48(4) . 4_665
Li7 Si5 Li7 89.04(6) 1_655 4_665
O51 Si5 Li12 53.04(6) . .
O52 Si5 Li12 123.033(18) . .
O52 Si5 Li12 123.034(18) 4_565 .
O53 Si5 Li12 53.41(6) . .
Li7 Si5 Li12 84.69(5) 1_655 .
Li7 Si5 Li12 84.69(5) 4_665 .
O51 Si5 Li11 41.28(4) . .
O52 Si5 Li11 91.20(3) . .
O52 Si5 Li11 91.20(3) 4_565 .
O53 Si5 Li11 147.73(4) . .
Li7 Si5 Li11 135.39(3) 1_655 .
Li7 Si5 Li11 135.39(3) 4_665 .
Li12 Si5 Li11 94.32(6) . .
O51 Si5 Li5 92.28(3) . 4_565
O52 Si5 Li5 93.12(3) . 4_565
O52 Si5 Li5 39.18(3) 4_565 4_565
O53 Si5 Li5 145.15(3) . 4_565
Li7 Si5 Li5 139.50(4) 1_655 4_565
Li7 Si5 Li5 93.71(4) 4_665 4_565
Li12 Si5 Li5 135.81(4) . 4_565
Li11 Si5 Li5 57.16(4) . 4_565
O51 Si5 Li5 92.28(3) . .
O52 Si5 Li5 39.18(3) . .
O52 Si5 Li5 93.11(3) 4_565 .
O53 Si5 Li5 145.15(3) . .
Li7 Si5 Li5 93.71(4) 1_655 .
Li7 Si5 Li5 139.50(4) 4_665 .
Li12 Si5 Li5 135.81(4) . .
Li11 Si5 Li5 57.16(4) . .
Li5 Si5 Li5 59.48(5) 4_565 .
O51 Si5 Li10 29.98(2) . 4_575
O52 Si5 Li10 84.82(3) . 4_575
O52 Si5 Li10 138.18(3) 4_565 4_575
O53 Si5 Li10 104.11(3) . 4_575
Li7 Si5 Li10 95.16(4) 1_655 4_575
Li7 Si5 Li10 142.26(4) 4_665 4_575
Li12 Si5 Li10 58.54(5) . 4_575
Li11 Si5 Li10 49.46(4) . 4_575
Li5 Si5 Li10 106.48(3) 4_565 4_575
Li5 Si5 Li10 77.75(3) . 4_575
O51 Si5 Li10 29.98(2) . 1_545
O52 Si5 Li10 138.18(3) . 1_545
O52 Si5 Li10 84.82(3) 4_565 1_545
O53 Si5 Li10 104.11(3) . 1_545
Li7 Si5 Li10 142.26(4) 1_655 1_545
Li7 Si5 Li10 95.16(4) 4_665 1_545
Li12 Si5 Li10 58.54(5) . 1_545
Li11 Si5 Li10 49.46(4) . 1_545
Li5 Si5 Li10 77.75(3) 4_565 1_545
Li5 Si5 Li10 106.48(3) . 1_545
Li10 Si5 Li10 59.97(5) 4_575 1_545
Si5 O51 Li10 125.00(4) . 4_575
Si5 O51 Li10 125.00(4) . 1_545
Li10 O51 Li10 109.99(8) 4_575 1_545
Si5 O51 Li12 85.99(7) . .
Li10 O51 Li12 92.16(6) 4_575 .
Li10 O51 Li12 92.16(6) 1_545 .
Si5 O51 Li11 107.25(6) . .
Li10 O51 Li11 80.34(5) 4_575 .
Li10 O51 Li11 80.34(5) 1_545 .
Li12 O51 Li11 166.76(8) . .
Si5 O52 Li16 126.14(5) . 4_565
Si5 O52 Li3 122.24(5) . .
Li16 O52 Li3 111.60(6) 4_565 .
Si5 O52 Li7 83.93(4) . 1_655
Li16 O52 Li7 95.64(6) 4_565 1_655
Li3 O52 Li7 92.18(7) . 1_655
Si5 O52 Li5 110.82(4) . .
Li16 O52 Li5 78.20(6) 4_565 .
Li3 O52 Li5 77.69(7) . .
Li7 O52 Li5 164.98(6) 1_655 .
Si5 O53 Li7 85.38(5) . 4_665
Si5 O53 Li7 85.38(5) . 1_655
Li7 O53 Li7 126.56(8) 4_665 1_655
Si5 O53 Li12 84.16(7) . .
Li7 O53 Li12 115.58(4) 4_665 .
Li7 O53 Li12 115.58(4) 1_655 .
Si5 O53 Li19 134.00(7) . .
Li7 O53 Li19 74.80(5) 4_665 .
Li7 O53 Li19 74.80(5) 1_655 .
Li12 O53 Li19 141.84(9) . .
Si5 O53 Li1 136.71(4) . 1_655
Li7 O53 Li1 137.64(6) 4_665 1_655
Li7 O53 Li1 72.46(5) 1_655 1_655
Li12 O53 Li1 73.38(6) . 1_655
Li19 O53 Li1 75.81(6) . 1_655
Si5 O53 Li1 136.71(4) . 4_665
Li7 O53 Li1 72.46(5) 4_665 4_665
Li7 O53 Li1 137.64(6) 1_655 4_665
Li12 O53 Li1 73.38(6) . 4_665
Li19 O53 Li1 75.81(6) . 4_665
Li1 O53 Li1 71.23(7) 1_655 4_665
O61 Si6 O63 113.31(3) . .
O61 Si6 O62 112.13(2) . 4_575
O63 Si6 O62 106.40(2) . 4_575
O61 Si6 O62 112.13(2) . .
O63 Si6 O62 106.40(2) . .
O62 Si6 O62 105.95(4) 4_575 .
O61 Si6 Li1 137.06(7) . 4_675
O63 Si6 Li1 53.53(4) . 4_675
O62 Si6 Li1 53.49(4) 4_575 4_675
O62 Si6 Li1 110.80(7) . 4_675
O61 Si6 Li1 137.06(7) . 1_655
O63 Si6 Li1 53.53(4) . 1_655
O62 Si6 Li1 110.80(7) 4_575 1_655
O62 Si6 Li1 53.49(4) . 1_655
Li1 Si6 Li1 73.03(12) 4_675 1_655
O61 Si6 Li18 135.79(7) . 3_666
O63 Si6 Li18 110.90(7) . 3_666
O62 Si6 Li18 53.304(19) 4_575 3_666
O62 Si6 Li18 53.304(19) . 3_666
Li1 Si6 Li18 72.93(8) 4_675 3_666
Li1 Si6 Li18 72.93(8) 1_655 3_666
O61 Si6 Li9 85.50(4) . 1_565
O63 Si6 Li9 147.24(3) . 1_565
O62 Si6 Li9 40.90(3) 4_575 1_565
O62 Si6 Li9 89.22(3) . 1_565
Li1 Si6 Li9 94.21(5) 4_675 1_565
Li1 Si6 Li9 128.80(6) 1_655 1_565
Li18 Si6 Li9 56.04(6) 3_666 1_565
O61 Si6 Li9 85.50(4) . 4_565
O63 Si6 Li9 147.24(3) . 4_565
O62 Si6 Li9 89.22(3) 4_575 4_565
O62 Si6 Li9 40.90(3) . 4_565
Li1 Si6 Li9 128.80(6) 4_675 4_565
Li1 Si6 Li9 94.21(5) 1_655 4_565
Li18 Si6 Li9 56.04(6) 3_666 4_565
Li9 Si6 Li9 55.40(5) 1_565 4_565
O61 Si6 Li7 86.17(3) . 1_655
O63 Si6 Li7 37.50(3) . 1_655
O62 Si6 Li7 143.17(3) 4_575 1_655
O62 Si6 Li7 95.08(3) . 1_655
Li1 Si6 Li7 91.03(5) 4_675 1_655
Li1 Si6 Li7 59.17(7) 1_655 1_655
Li18 Si6 Li7 132.08(6) 3_666 1_655
Li9 Si6 Li7 171.58(5) 1_565 1_655
Li9 Si6 Li7 125.08(4) 4_565 1_655
O61 Si6 Li7 86.17(3) . 4_675
O63 Si6 Li7 37.50(3) . 4_675
O62 Si6 Li7 95.08(3) 4_575 4_675
O62 Si6 Li7 143.17(3) . 4_675
Li1 Si6 Li7 59.17(7) 4_675 4_675
Li1 Si6 Li7 91.03(5) 1_655 4_675
Li18 Si6 Li7 132.08(6) 3_666 4_675
Li9 Si6 Li7 125.08(4) 1_565 4_675
Li9 Si6 Li7 171.58(5) 4_565 4_675
Li7 Si6 Li7 52.96(5) 1_655 4_675
O61 Si6 Li10 33.10(3) . .
O63 Si6 Li10 123.87(3) . .
O62 Si6 Li10 79.10(3) 4_575 .
O62 Si6 Li10 126.11(3) . .
Li1 Si6 Li10 113.88(7) 4_675 .
Li1 Si6 Li10 170.05(8) 1_655 .
Li18 Si6 Li10 115.41(6) 3_666 .
Li9 Si6 Li10 59.39(4) 1_565 .
Li9 Si6 Li10 86.79(4) 4_565 .
Li7 Si6 Li10 112.39(4) 1_655 .
Li7 Si6 Li10 86.92(3) 4_675 .
Si6 O61 Li10 119.64(5) . 4_575
Si6 O61 Li10 119.64(5) . .
Li10 O61 Li10 101.80(8) 4_575 .
Si6 O61 Li3 118.86(7) . .
Li10 O61 Li3 95.98(6) 4_575 .
Li10 O61 Li3 95.98(6) . .
Si6 O62 Li9 105.14(5) . 4_565
Si6 O62 Li1 85.78(5) . 1_655
Li9 O62 Li1 167.48(7) 4_565 1_655
Si6 O62 Li12 111.06(5) . .
Li9 O62 Li12 94.39(7) 4_565 .
Li1 O62 Li12 87.16(10) 1_655 .
Si6 O62 Li18 88.92(4) . 3_666
Li9 O62 Li18 78.95(9) 4_565 3_666
Li1 O62 Li18 95.43(12) 1_655 3_666
Li12 O62 Li18 160.00(6) . 3_666
Si6 O62 Li18 171.31(8) . 1_655
Li9 O62 Li18 82.91(9) 4_565 1_655
Li1 O62 Li18 85.88(9) 1_655 1_655
Li12 O62 Li18 70.90(7) . 1_655
Li18 O62 Li18 89.47(2) 3_666 1_655
Si6 O63 Li7 111.80(5) . 1_655
Si6 O63 Li7 111.80(5) . 4_675
Li7 O63 Li7 85.68(8) 1_655 4_675
Si6 O63 Li1 85.94(5) . 4_675
Li7 O63 Li1 162.25(7) 1_655 4_675
Li7 O63 Li1 87.06(9) 4_675 4_675
Si6 O63 Li1 85.94(5) . 1_655
Li7 O63 Li1 87.06(9) 1_655 1_655
Li7 O63 Li1 162.25(7) 4_675 1_655
Li1 O63 Li1 95.12(18) 4_675 1_655
Si6 O63 Li13 167.11(7) . 1_655
Li7 O63 Li13 77.23(6) 1_655 1_655
Li7 O63 Li13 77.23(6) 4_675 1_655
Li1 O63 Li13 85.38(6) 4_675 1_655
Li1 O63 Li13 85.38(6) 1_655 1_655
O73 Si7 O72 109.65(4) . .
O73 Si7 O71 112.73(2) . 4_575
O72 Si7 O71 107.48(2) . 4_575
O73 Si7 O71 112.73(2) . .
O72 Si7 O71 107.48(2) . .
O71 Si7 O71 106.49(3) 4_575 .
O73 Si7 Li15 50.74(5) . .
O72 Si7 Li15 58.91(5) . .
O71 Si7 Li15 126.750(17) 4_575 .
O71 Si7 Li15 126.751(17) . .
O73 Si7 Li14 143.86(4) . .
O72 Si7 Li14 54.87(4) . .
O71 Si7 Li14 103.35(4) 4_575 .
O71 Si7 Li14 55.93(3) . .
Li15 Si7 Li14 105.15(5) . .
O73 Si7 Li14 143.86(4) . 4_575
O72 Si7 Li14 54.87(4) . 4_575
O71 Si7 Li14 55.93(3) 4_575 4_575
O71 Si7 Li14 103.35(4) . 4_575
Li15 Si7 Li14 105.15(5) . 4_575
Li14 Si7 Li14 59.16(6) . 4_575
O73 Si7 Li13 137.13(6) . .
O72 Si7 Li13 113.22(6) . .
O71 Si7 Li13 53.554(18) 4_575 .
O71 Si7 Li13 53.554(18) . .
Li15 Si7 Li13 172.13(7) . .
Li14 Si7 Li13 68.13(5) . .
Li14 Si7 Li13 68.13(5) 4_575 .
O73 Si7 Li7 87.06(4) . 4_575
O72 Si7 Li7 148.03(3) . 4_575
O71 Si7 Li7 40.71(3) 4_575 4_575
O71 Si7 Li7 89.50(3) . 4_575
Li15 Si7 Li7 130.59(5) . 4_575
Li14 Si7 Li7 123.85(4) . 4_575
Li14 Si7 Li7 95.47(4) 4_575 4_575
Li13 Si7 Li7 55.76(5) . 4_575
O73 Si7 Li7 87.06(4) . .
O72 Si7 Li7 148.03(3) . .
O71 Si7 Li7 89.50(3) 4_575 .
O71 Si7 Li7 40.71(3) . .
Li15 Si7 Li7 130.59(5) . .
Li14 Si7 Li7 95.47(4) . .
Li14 Si7 Li7 123.85(4) 4_575 .
Li13 Si7 Li7 55.76(5) . .
Li7 Si7 Li7 55.77(5) 4_575 .
O73 Si7 Li16 34.63(3) . 4_465
O72 Si7 Li16 122.07(3) . 4_465
O71 Si7 Li16 126.53(3) 4_575 4_465
O71 Si7 Li16 78.11(3) . 4_465
Li15 Si7 Li16 71.84(5) . 4_465
Li14 Si7 Li16 120.32(4) . 4_465
Li14 Si7 Li16 176.84(4) 4_575 4_465
Li13 Si7 Li16 114.79(5) . 4_465
Li7 Si7 Li16 87.32(4) 4_575 4_465
Li7 Si7 Li16 59.04(4) . 4_465
O73 Si7 Li16 34.63(3) . 1_465
O72 Si7 Li16 122.07(3) . 1_465
O71 Si7 Li16 78.11(3) 4_575 1_465
O71 Si7 Li16 126.53(3) . 1_465
Li15 Si7 Li16 71.84(5) . 1_465
Li14 Si7 Li16 176.84(4) . 1_465
Li14 Si7 Li16 120.32(4) 4_575 1_465
Li13 Si7 Li16 114.79(5) . 1_465
Li7 Si7 Li16 59.04(4) 4_575 1_465
Li7 Si7 Li16 87.32(4) . 1_465
Li16 Si7 Li16 60.01(5) 4_465 1_465
Si7 O71 Li7 105.39(5) . .
Si7 O71 Li15 109.92(5) . 3_565
Li7 O71 Li15 101.15(7) . 3_565
Si7 O71 Li13 88.15(4) . .
Li7 O71 Li13 78.59(8) . .
Li15 O71 Li13 161.03(6) 3_565 .
Si7 O71 Li19 172.71(9) . 1_455
Li7 O71 Li19 81.57(10) . 1_455
Li15 O71 Li19 70.13(7) 3_565 1_455
Li13 O71 Li19 91.21(6) . 1_455
Si7 O71 Li14 84.78(4) . .
Li7 O71 Li14 161.46(6) . .
Li15 O71 Li14 89.47(7) 3_565 .
Li13 O71 Li14 86.44(8) . .
Li19 O71 Li14 87.94(10) 1_455 .
Si7 O72 Li16 128.64(4) . 2_655
Si7 O72 Li16 128.64(4) . 3_665
Li16 O72 Li16 101.03(8) 2_655 3_665
Si7 O72 Li14 86.51(4) . .
Li16 O72 Li14 70.65(5) 2_655 .
Li16 O72 Li14 126.77(6) 3_665 .
Si7 O72 Li14 86.52(4) . 4_575
Li16 O72 Li14 126.77(6) 2_655 4_575
Li16 O72 Li14 70.65(5) 3_665 4_575
Li14 O72 Li14 74.10(8) . 4_575
Si7 O72 Li15 80.88(6) . .
Li16 O72 Li15 88.87(5) 2_655 .
Li16 O72 Li15 88.87(5) 3_665 .
Li14 O72 Li15 140.91(4) . .
Li14 O72 Li15 140.91(4) 4_575 .
Si7 O73 Li16 116.97(5) . 4_465
Si7 O73 Li16 116.97(5) . 1_465
Li16 O73 Li16 103.29(8) 4_465 1_465
Si7 O73 Li15 89.06(7) . .
Li16 O73 Li15 115.52(5) 4_465 .
Li16 O73 Li15 115.52(5) 1_465 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Li1 O62 2.0410(17) 1_455
Li1 O63 2.0417(17) 1_455
Li1 O33 2.0458(16) .
Li1 O32 2.0496(17) .
Li1 Si6 2.5324(16) 1_455
Li1 Si3 2.5403(16) .
Li1 O43 2.558(3) 3_666
Li1 O53 2.649(3) 1_455
Li1 Li9 2.709(3) 2_656
Li1 Li6 2.760(3) 3_666
Li1 Li7 2.762(3) .
Li1 Li12 2.822(3) 1_455
Li2 O31 1.9013(13) .
Li2 O41 1.9394(13) 3_666
Li2 O23 1.9625(13) .
Li2 O42 2.0006(14) .
Li2 Li10 2.480(2) 4_575
Li2 Li8 2.5058(19) 3_666
Li2 Li4 2.7784(18) .
Li2 Li6 2.806(2) 3_666
Li2 Li8 2.8924(19) .
Li2 Si4 2.9793(13) .
Li2 Li2 2.985(2) 4_565
Li2 Si3 3.0175(13) .
Li3 O61 1.9201(19) .
Li3 O52 1.9718(10) 4_575
Li3 O52 1.9718(10) .
Li3 O21 2.074(2) .
Li3 Li5 2.5263(19) 4_575
Li3 Li5 2.5264(19) .
Li3 Li10 2.8421(19) 4_575
Li3 Li10 2.8421(19) .
Li3 Li7 2.862(2) 4_675
Li3 Li7 2.862(2) 1_655
Li3 Si2 2.9723(19) .
Li3 Si6 3.0339(19) .
Li4 O23 1.9352(14) .
Li4 O13 1.9405(14) .
Li4 O32 1.9552(13) .
Li4 O22 1.9812(13) .
Li4 Li14 2.4022(18) .
Li4 Si2 2.4522(12) .
Li4 Li4 2.619(3) 4_565
Li4 Li19 2.688(3) 1_455
Li4 Li13 2.803(2) .
Li4 Li11 2.812(2) .
Li4 Si3 2.8381(12) .
Li5 O11 1.8793(13) .
Li5 O21 1.9323(13) .
Li5 O12 1.9742(13) 3_665
Li5 O52 2.0547(13) .
Li5 Li16 2.5017(19) 4_565
Li5 Li17 2.757(2) 3_665
Li5 Li17 2.770(2) .
Li5 Li11 2.8748(19) .
Li5 Li5 3.016(2) 4_565
Li5 Si5 3.0401(13) .
Li5 Si1 3.0437(13) .
Li6 O41 1.947(2) .
Li6 O43 2.003(2) .
Li6 O32 2.0323(11) 3_666
Li6 O32 2.0323(11) 2_646
Li6 Li13 2.402(3) 3_666
Li6 Si4 2.4540(19) .
Li6 Li1 2.760(3) 3_666
Li6 Li1 2.760(3) 2_646
Li6 Li2 2.806(2) 2_646
Li6 Li2 2.806(2) 3_666
Li6 Li4 2.928(2) 3_666
Li6 Li4 2.928(2) 2_646
Li7 O53 1.9160(13) 1_455
Li7 O71 1.9353(13) .
Li7 O63 1.9675(14) 1_455
Li7 O52 2.0002(15) 1_455
Li7 Si5 2.4409(13) 1_455
Li7 Li13 2.591(2) .
Li7 Li7 2.676(3) 4_575
Li7 Li19 2.677(3) 1_455
Li7 Si7 2.8608(13) .
Li7 Li3 2.862(2) 1_455
Li7 Li16 2.8966(19) 4_465
Li8 O31 1.9110(19) .
Li8 O42 1.9728(10) 3_666
Li8 O42 1.9728(10) 2_646
Li8 O41 2.0074(19) .
Li8 Li2 2.5058(19) 3_666
Li8 Li2 2.5058(19) 2_646
Li8 Li9 2.847(2) 3_656
Li8 Li9 2.847(2) 2_656
Li8 Li2 2.8923(19) 4_565
Li8 Si4 2.9613(18) .
Li8 Si3 2.9628(18) .
Li9 O43 1.9315(14) .
Li9 O62 1.9420(13) 4_565
Li9 O33 1.9570(14) 3_656
Li9 O42 1.9942(15) 4_565
Li9 Si4 2.4509(13) .
Li9 Li18 2.619(3) 3_656
Li9 Li9 2.662(3) 4
Li9 Li1 2.708(3) 2_646
Li9 Li18 2.746(3) 1_655
Li9 Li8 2.847(2) 3_656
Li9 Si6 2.8631(13) 1_545
Li9 Li10 2.924(2) 1_545
Li10 O61 1.9049(13) .
Li10 O51 1.9179(13) 1_565
Li10 O42 1.9431(13) 4_575
Li10 O23 1.9988(14) 4_575
Li10 Li2 2.480(2) 4_575
Li10 Li11 2.5616(19) 1_565
Li10 Li12 2.806(2) 1_565
Li10 Li9 2.924(2) 1_565
Li10 Li10 2.957(2) 4_575
Li10 Si2 3.0188(13) .
Li10 Si6 3.0323(13) .
Li11 O11 1.9600(19) .
Li11 O23 1.9916(10) .
Li11 O23 1.9917(10) 4_565
Li11 O51 2.050(2) .
Li11 Li10 2.5616(19) 4_575
Li11 Li10 2.5616(19) 1_545
Li11 Li4 2.812(2) 4_565
Li11 Li5 2.8747(19) 4_565
Li11 Si1 2.9108(19) .
Li11 Si5 2.9680(19) .
Li12 O51 1.978(2) .
Li12 O53 1.993(2) .
Li12 O62 2.0532(12) .
Li12 O62 2.0532(12) 4_565
Li12 Li18 2.467(3) 1_655
Li12 Si5 2.469(2) .
Li12 Li10 2.806(2) 1_545
Li12 Li10 2.806(2) 4_575
Li12 Li1 2.822(3) 1_655
Li12 Li1 2.822(3) 4_665
Li12 Li9 2.932(2) 4_565
Li13 O71 2.1482(17) .
Li13 O71 2.1482(17) 4_575
Li13 O32 2.1751(14) .
Li13 O32 2.1751(14) 4_575
Li13 O63 2.177(3) 1_455
Li13 Li6 2.402(3) 3_666
Li13 O22 2.518(3) .
Li13 Li7 2.591(2) 4_575
Li13 Si7 2.669(2) .
Li13 Li4 2.803(2) 4_575
Li14 O12 1.9968(14) .
Li14 O22 2.0330(16) .
Li14 O13 2.0443(14) .
Li14 O72 2.1326(14) .
Li14 O71 2.1650(14) .
Li14 Li16 2.3917(18) 2_655
Li14 Si1 2.5311(13) .
Li14 Li14 2.570(3) 4_575
Li14 Si7 2.6027(14) .
Li14 Li17 2.679(2) .
Li15 O73 1.927(2) .
Li15 O71 2.0640(12) 3_565
Li15 O71 2.0640(12) 2
Li15 O72 2.159(2) .
Li15 Li19 2.425(3) 3_665
Li15 Si7 2.4892(19) .
Li15 Li16 2.914(2) 3_665
Li15 Li16 2.914(2) 2_655
Li15 Li14 2.977(2) 3_565
Li15 Li14 2.977(2) 2
Li15 Si7 3.05398(15) 3_565
Li15 Si7 3.05398(16) 3_575
Li16 O52 1.9077(13) 4_565
Li16 O73 1.9204(13) 1_645
Li16 O12 1.9721(14) 2_645
Li16 O72 1.9996(13) 3_665
Li16 Li14 2.3917(18) 2_645
Li16 Li5 2.5017(19) 4_565
Li16 Li7 2.8965(19) 4_665
Li16 Li15 2.914(2) 3_665
Li16 Si7 3.0116(13) 1_645
Li16 Li16 3.012(2) 4
Li16 Li16 3.087(2) 4_565
Li16 Si1 3.1395(13) 3_655
Li17 O12 1.9227(11) .
Li17 O12 1.9227(11) 4_575
Li17 O21 2.047(2) .
Li17 O22 2.499(2) .
Li17 Li14 2.679(2) 4_575
Li17 Li5 2.757(2) 3_665
Li17 Li5 2.757(2) 2_655
Li17 Si2 2.758(2) .
Li17 Li5 2.770(2) 4_575
Li17 Si1 3.1051(5) 1_565
Li18 O62 2.169(2) 3_666
Li18 O62 2.169(2) 2_646
Li18 O62 2.1954(15) 4_465
Li18 O62 2.1954(15) 1_455
Li18 O33 2.255(3) .
Li18 Li12 2.467(3) 1_455
Li18 O43 2.513(3) 1_455
Li18 Li9 2.619(3) 2_656
Li18 Li9 2.619(3) 3_656
Li18 Si6 2.704(2) 3_666
Li18 Li9 2.746(3) 1_455
Li18 Li9 2.746(3) 4_465
Li19 O71 2.1555(16) 4_665
Li19 O71 2.1555(16) 1_655
Li19 O32 2.169(2) 1_655
Li19 O32 2.169(2) 4_665
Li19 Li15 2.425(3) 3_665
Li19 O53 2.439(3) .
Li19 O13 2.443(3) 1_655
Li19 Li7 2.677(3) 4_665
Li19 Li7 2.677(3) 1_655
Li19 Li4 2.688(3) 1_655
Li19 Li4 2.688(3) 4_665
Li19 Si3 2.691(2) 1_655
Si1 O11 1.6146(7) .
Si1 O12 1.6328(4) 4_565
Si1 O12 1.6328(4) .
Si1 O13 1.6779(6) .
Si1 Li14 2.5310(13) 4_565
Si1 Li5 3.0437(13) 4_565
Si1 Li17 3.1051(5) 1_545
Si1 Li5 3.1314(12) 2_645
O11 Li5 1.8793(13) 4_565
O12 Li16 1.9722(14) 2_655
O12 Li5 1.9741(13) 3_665
O13 Li4 1.9406(14) 4_565
O13 Li14 2.0443(14) 4_565
O13 Li19 2.443(3) 1_455
Si2 O21 1.6245(6) .
Si2 O23 1.6334(4) .
Si2 O23 1.6334(4) 4_575
Si2 O22 1.6746(7) .
Si2 Li4 2.4522(12) 4_575
Si2 Li10 3.0188(13) 4_575
Si2 Li11 3.1523(5) 1_565
O21 Li5 1.9323(13) 4_575
O22 Li4 1.9812(13) 4_575
O22 Li14 2.0331(16) 4_575
O23 Li10 1.9988(14) 4_575
Si3 O31 1.5997(7) .
Si3 O33 1.6500(6) .
Si3 O32 1.6534(5) 4_565
Si3 O32 1.6534(5) .
Si3 Li1 2.5403(16) 4_565
Si3 Li19 2.691(2) 1_455
Si3 Li4 2.8381(12) 4_565
Si3 Li2 3.0175(13) 4_565
O31 Li2 1.9013(13) 4_565
O32 Li6 2.0324(11) 3_666
O32 Li19 2.169(2) 1_455
O33 Li9 1.9571(14) 2_656
O33 Li9 1.9571(14) 3_656
O33 Li1 2.0458(17) 4_565
Si4 O42 1.6265(4) 4_565
Si4 O42 1.6265(5) .
Si4 O41 1.6271(6) .
Si4 O43 1.6748(7) .
Si4 Li9 2.4509(13) 4_565
Si4 Li2 2.9792(13) 4_565
Si4 Li8 3.1498(5) 3_656
Si4 Li8 3.1498(5) 3_666
O41 Li2 1.9395(13) 3_666
O41 Li2 1.9395(13) 2_646
O42 Li10 1.9430(13) 4_575
O42 Li8 1.9728(10) 3_666
O42 Li9 1.9942(15) 4_565
O43 Li9 1.9315(14) 4_565
O43 Li18 2.513(3) 1_655
O43 Li1 2.558(3) 3_666
O43 Li1 2.558(3) 2_646
Si5 O51 1.6226(6) .
Si5 O52 1.6264(5) .
Si5 O52 1.6265(5) 4_565
Si5 O53 1.6745(7) .
Si5 Li7 2.4409(13) 1_655
Si5 Li7 2.4409(13) 4_665
Si5 Li5 3.0401(13) 4_565
Si5 Li10 3.1435(13) 4_575
Si5 Li10 3.1435(13) 1_545
O51 Li10 1.9179(13) 4_575
O51 Li10 1.9179(13) 1_545
O52 Li16 1.9078(13) 4_565
O52 Li7 2.0001(15) 1_655
O53 Li7 1.9160(13) 4_665
O53 Li7 1.9160(13) 1_655
O53 Li1 2.649(3) 1_655
O53 Li1 2.649(3) 4_665
Si6 O61 1.5984(6) .
Si6 O63 1.6498(6) .
Si6 O62 1.6569(5) 4_575
Si6 O62 1.6569(5) .
Si6 Li1 2.5324(16) 4_675
Si6 Li1 2.5324(16) 1_655
Si6 Li18 2.704(2) 3_666
Si6 Li9 2.8632(13) 1_565
Si6 Li9 2.8632(13) 4_565
Si6 Li7 3.0007(13) 1_655
Si6 Li7 3.0007(13) 4_675
O61 Li10 1.9049(13) 4_575
O62 Li9 1.9420(13) 4_565
O62 Li1 2.0410(17) 1_655
O62 Li18 2.169(2) 3_666
O62 Li18 2.1955(15) 1_655
O63 Li7 1.9675(14) 1_655
O63 Li7 1.9675(14) 4_675
O63 Li1 2.0417(17) 4_675
O63 Li1 2.0417(17) 1_655
O63 Li13 2.177(3) 1_655
Si7 O73 1.6070(7) .
Si7 O72 1.6272(6) .
Si7 O71 1.6549(5) 4_575
Si7 O71 1.6549(5) .
Si7 Li14 2.6027(14) 4_575
Si7 Li7 2.8608(13) 4_575
Si7 Li16 3.0116(13) 4_465
Si7 Li16 3.0116(13) 1_465
O71 Li15 2.0640(12) 3_565
O71 Li19 2.1554(16) 1_455
O72 Li16 1.9996(13) 2_655
O72 Li16 1.9996(13) 3_665
O72 Li14 2.1326(14) 4_575
O73 Li16 1.9204(13) 4_465
O73 Li16 1.9204(13) 1_465
#BEGIN Loops that were not found in dictionaries:
loop_
_publcif_info_datablock.id
_publcif_info_datablock.publ_exptl
_publcif_info_datablock.publ_geom
_publcif_info_datablock.structure
{a5b76c70-cd17-4a7c-af5b-b3e894aabd62} ? ? ?
{f64d6a86-4e12-4441-aeca-efe3daffc3db} y y y
loop_
_publcif_info_exptl_table_extra_item
sin_theta_over_lambda_max
loop_
_publcif_info_tables.block_id
_publcif_info_tables.reference_item
{a5b76c70-cd17-4a7c-af5b-b3e894aabd62} '_publcif_info_datablock.publ_exptl'
#END Loops that were not found in dictionaries
